Chemical Science View Article Online

EDGE ARTICLE

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Cite this: Chem. Sci., 2013, 4, 139

View Journal | View Issue

A theoretical analysis of chemical bonding, vibronic coupling, and magnetic anisotropy in linear iron(II) complexes with single-molecule magnet behavior† Mihail Atanasov,*ab Joseph M. Zadrozny,c Jeﬀrey R. Longc and Frank Neese*a The electronic structure and magnetic anisotropy of six complexes of high-spin FeII with linear FeX2 (X ¼ C, N, O) cores, Fe[N(SiMe3)(Dipp)]2 (1), Fe[C(SiMe3)3]2 (2), Fe[N(H)Ar0 ]2 (3), Fe[N(H)Ar*]2 (4), Fe[O(Ar0 )]2 (5), and Fe[N(t-Bu)2]2 (7) [Dipp ¼ C6H3-2,6-Pri2; Ar0 ¼ C6H3-2,6-(C6H3-2,6-Pri2)2; Ar* ¼ C6H3-2,6-(C6H2-2,4,6Pri2)2; Ar# ¼ C6H3-2,6-(C6H2-2,4,6-Me3)2], and one bent (FeN2) complex, Fe[N(H)Ar#]2 (6), have been studied theoretically using complete active space self-consistent ﬁeld (CASSCF) wavefunctions in conjunction with N-Electron Valence Perturbation Theory (NEVPT2) and quasidegenerate perturbation ¨ ssbauer theory (QDPT) for the treatment of magnetic ﬁeld and spin-dependent relativistic eﬀects. Mo studies on compound 2 indicate an internal magnetic ﬁeld of unprecedented magnitude (151.7 T) at the FeII nucleus. This has been interpreted as arising from ﬁrst order angular momentum of the 5D ground state of FeII center (J. Am. Chem. Soc. 2004, 126, 10206). Using geometries from X-ray structural data, ligand ﬁeld parameters for the Fe-ligand bonds were extracted using a 1 : 1 mapping of the angular overlap model onto multireference wavefunctions. The results demonstrate that the metal– ligand bonding in these complexes is characterized by: (i) strong 3dz2–4s mixing (in all complexes), (ii) pbonding anisotropy involving the strong p-donor amide ligands (in 1, 3–4, 6, and 7) and (iii) orbital mixings of the s–p type for Fe–O bonds (misdirected valence in 5). The interplay of all three eﬀects leads to an appreciable symmetry lowering and splitting of the 5D (3dxy, 3dx2y2) ground state. The strengths of the eﬀects increase in the order 1 < 5 < 7 6. However, the diﬀerential bonding eﬀects are largely overruled by ﬁrst-order spin–orbit coupling, which leads to a nearly non-reduced orbital contribution of L ¼ 1 to yield a net magnetic moment of about 6 mB. This unique spin–orbital driven magnetism is signiﬁcantly modulated by geometric distortion eﬀects: static distortions for the bent complex 6 and dynamic vibronic coupling eﬀects of the Renner–Teller type of increasing strength for the series 1–5. Ab initio calculations based on geometries from X-ray data for 1 and 2 reproduce the magnetic data exceptionally well. Magnetic sublevels and wavefunctions were calculated employing a dynamic Renner–Teller vibronic coupling model with vibronic coupling parameters adjusted from the ab initio results on a small Fe(CH3)2 truncated model complex. The model reproduces the observed reduction of the orbital moments and quantitatively reproduces the magnetic susceptibility data of 3–5 after introduction of the vibronic coupling strength (f) as a single adjustable parameter. Its value varies

Received 30th August 2012 Accepted 3rd October 2012

in a narrow range (f ¼ 0.142 0.015) across the series. The results indicate that the systems are near the borderline of the transition from a static to a dynamic Renner–Teller eﬀect. Renner–Teller vibronic activity is used to explain the large reduction of the spin-reversal barrier Ueﬀ along the series from 1 to

DOI: 10.1039/c2sc21394j

5. Based upon the theoretical analysis, guidelines for generating new single-molecule magnets with

www.rsc.org/chemicalscience

enhanced magnetic anisotropies and longer relaxation times are formulated.

a Max-Planck Institut fur Chemische Energiekonversion, Stifstr. 32–34, D-45470 Mulheim an der Ruhr, Germany. E-mail: [email protected]; frank. [email protected] b

Institute of General and Inorganic Chemistry, Bulgarian Academy of Sciences, Acad Georgi Bontchev Str. 11, 1113 Soa, Bulgaria

c

Department of Chemistry, University of California, Berkeley, CA, 94720, USA

† Electronic supplementary information (ESI) available: Full computational details, results, and formulae. Calculated molar dc susceptibility and magnetization data for 2–5 and NIR d–d absorption spectrum of 1. See DOI: 10.1039/c2sc21394j

This journal is ª The Royal Society of Chemistry 2013

1

Introduction

Considerable eﬀorts have been dedicated toward the synthesis and characterization of single-molecule magnets—paramagnetic molecules displaying magnetic bistability. The motivation for these studies lies in the interest in the potential future applications for such compounds in high-density information storage,1 quantum computing,2–4 and magnetic refrigeration.5 Single-molecule magnets are open shell spin systems,

Chem. Sci., 2013, 4, 139–156 | 139

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science which under an applied external direct current (dc) magnetic eld are magnetized and remain so upon removal of the eld. The phenomenon occurs at temperatures below a critical value, the blocking temperature TB. This property is intrinsically related to the existence of an energy barrier U ¼ S2|D| for the reversal of the magnetization (D is the axial zero-eld splitting parameter for the ground state of total spin S, frequently referred to as the magnetic anisotropy) by spin–phonon coupling and/or thermally assisted quantum tunneling, which usually renders the eﬀective barrier Ueﬀ smaller than U. The targeted large and negative quantity D implies orbital contributions to the spin from spin–orbit coupling in combination with an axial threefold or fourfold molecular symmetry (uniaxial anisotropy). Since the discovery of the eﬀect in the celebrated Mn12 single-molecule magnet (TB z 3.5 K, Ueﬀ up to 72 K),6–8 many such systems belonging to the same family or other ones – (e.g., Mn6,9 Fe8,10 Mn4,11 and Fe4 (ref. 12–14) have been found to exhibit a similar type of magnetic behavior. It was pointed out that, with the number of spin centers being the same, since rDr f 1/S2, a high value of S is not a necessary condition for large Ueﬀ values to occur.15 It is important to note that this mathematical relationship is not a feature that arises from cluster spin coupling,16 but instead follows from the fundamental theory of the zero-eld splitting interaction.17 This prediction is supported by experiment, as comparison between D values of Mnn complexes with diﬀerent nuclearity (n) and variable spinground states (S) shows: n ¼ 1, D ¼ 2.29 cm1, S ¼ 2,16 n ¼ 6, D ¼ 1.22 cm1, S ¼ 4 (ref. 18), n ¼ 12, D ¼ 0.5 cm1, S ¼ 10,6–8 n ¼ 6, D ¼ 0.43 cm1, S ¼ 12,9 and n ¼ 18, D ¼ 0.13 cm1, S ¼ 13.19 However, in favor of systems with a large total spin, one can quote that the relaxation time (s) for the thermally activated process is greatly enhanced by large values of S, as was pointed out on theoretical grounds (s f (S6/U3)exp(U/kBT)).20,7 It has been also shown (ref. 7, Chapter 6) that increasing total spin S leads to suppression of the quantum tunneling of the magnetization as quantied by the ground state (Landau–Zener) splitting DE(MS ¼ S) which vanishes exponentially with DE (MS ¼ S) f [Hx/(4rDrS)]2S, Hx – the intrinsic transversal magnetic eld. In MnIII- and FeIII-based single-molecule magnets, the magnetic anisotropy arises from favorable alignment of local Dtensors, which originate from mixing, via spin–orbit coupling, of the non-degenerate ground states of MnIII (d4, subject to static Jahn–Teller distortions) or of FeIII (d5) with excited electronic states bearing rst-order orbital angular momenta. The directed, favorable alignment of local anisotropy axes in a multinuclear transition metal complex is obviously a grand synthetic challenge that cannot be considered as being solved. Hence, another strategy to achieve more negative D-values is to focus on complexes with trigonal geometries and orbitally degenerate ground states 2S+1E. Hybrid ligand scaﬀolds of FeII with trianionic tris(pyrrolyl-a-methyl) amines (tpa),21 for example, enforce a three-fold coordination geometry around the FeII centers, which can result in unusually large values, such as D ¼ 40 cm1 for [K(DME)4][Fe(tpaMes)].22 The observation of slow relaxation of the magnetization in this complex with the presence of a small dc eld, with an eﬀective relaxation barrier 140 | Chem. Sci., 2013, 4, 139–156

Edge Article of Ueﬀ ¼ 42 cm1, provided the rst example of a mononuclear transition metal complex with single-molecule magnet-like behavior.22 Expanding on this discovery, a series of four structurally and magnetically well-documented compounds: [Fe(tpaR)] (R ¼ tert-butyl, mesityl, phenyl and 2,6-diuorophenyl) were reported to display similar properties tuned by a variation of the substituents R.23 In the trigonally elongated site imposed by the tpaR ligand, the (dxz,yz)1 electron conguration24 yields a contribution of ML ¼ 1 to the net spin moment of MS ¼ 2, resulting in a bistable MJ ¼ 3 (5/2 mB) ground state.25 The eﬀect of the orbital moment on the magnetic anisotropy would be enhanced in hypothetical trigonally compressed tetrahedral FeX4 (5E(dx2y2,xy)1)26 or linear FeX2 (5D(dx2y2,xy)1) complexes possessing a twice larger orbital contribution to the magnetic moment of ML ¼ 2.27 In one complex of the latter type, Fe [C(SiMe3)3]2 (2), very large orbital momentum contributions, equivalent to adding two full S ¼ 1/2 spins to the spin-only value of S ¼ 2, were demonstrated by an unusually large internal hyperne eld (Hint ¼ 151.6 T), as manifested in the M¨ ossbauer spectra and also by dc magnetization measurement.28 A similar but less pronounced hyperne eld (Hint ¼ 105 T) was later found in the compound Fe[N(t-Bu)2]2 (7), with the lower relative magnitude of Hint being attributed to the lower eﬀective symmetry imposed by the non-axially symmetric ligands.29 Additionally, experimental observation of quenched orbital angular momentum induced by a bent L–Fe–L angle was shown for the two-coordinate complex Fe[N(H)Ar#]2 (Ar# ¼ C6H3-2,6(C6H2-2,4,6-Me3)2) (6), in contrast to the linear Fe[N(H)Ar*]2 analogue (Ar* ¼ C6H3-2,6-(C6H2-2,4,6-Pri2)2) (4), which showed the large magnetic moment and internal hyperne eld suggestive of orbital angular momentum.30 Transition metal complexes with open d-shells have traditionally been treated by ligand eld theory (LFT). As a parametrical model, LFT can only be used for the sake of interpretation, rather than for the prediction of properties. Density functional theory (DFT), being broadly used in chemistry for the prediction of ground state geometries and properties of electronic states in molecules, is well suited for systems with orbitally non-degenerate ground states (mono-determinantal wavefunctions). In contrast, the applicability of the theory is severely limited in cases where a superposition of charge distributions described by several rather than one Slater determinants (multi-determinantal wavefunctions) is mandatory for a realistic description. Systems with orbital degeneracy, which are the subject of the present study, clearly fall into this latter category. In this context, we mention, but will not further discuss, pragmatic approaches that allow one to deduce ligand eld parameters from DFT calculations.31–34 Magnetic systems of the type considered here are still too large to be treated with the available implementations of variational conguration interaction (CI) type approaches that cover both static and dynamic correlation eﬀects. Even the application of complete active space self-consistent eld method (CASSCF)35 in conjunction with second-order perturbation corrections to the CASSCF energies (such as the complete active space perturbation theory, CASPT2,36–40 or the N-electron-Valence-Perturbation Theory NEVPT2 (ref. 40–44)) are very challenging to apply to

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article systems with more than one hundred atoms in conjunction with at least triple-zeta basis sets. The potential of using such approaches to calculate spin Hamiltonian parameters of mono-15,45–47 and bi-48–50 and even trinuclear transition metal complexes51 was recently demonstrated. Additionally, a general rst-principles method to calculate the spin-dependent part of the energies of ground and excited multiplets for larger polynuclear complexes was proposed.52 In this study, we apply the recent implementation of the CASSCF and NEVPT2 methods in the ORCA53,54 program package to perform large-scale correlated calculations on the electronic structure and magnetic properties of a series of complexes of high-spin FeII with linear FeX2 (1–5, 7) and bent FeN2 (6) cores (see ref. 29 and 55 for depictions of the structures of these molecules). This work was performed in parallel with an ongoing experimental study of their magnetic properties reported in the preceding companion paper.55 We use the protocol developed and applied for the interpretation, analysis, and prediction of the magnetic properties of the closely related series of [Fe(tpaR)] compounds published recently.46 The energies of the lowest spin-levels, which govern the magnetic behavior of the complexes, and their ligand eld analysis provide important insights into the respective inuences of chemical bonding and static and dynamic vibronic coupling on the observed spin-reversal barriers. This paper is divided into two parts. In the rst part, the basic theory and the computational scheme are outlined. These include the ligand eld background for analyzing the ab initio results and the static and dynamic vibronic coupling model employed for the interpretation of the magnetic data. In the second part, the results involving analysis of the chemical bonding, magnetic properties, and the ligand eld are described.

2

Computations and theory

2.1

Computations

The electronic energy levels for the complexes were computed using geometries from the crystal structures of 1 and 3,55 2,56 4 and 6,30 5,57 and 7.29 The computational protocol for the calculation of CASSCF/NEVPT2 wavefunctions/energies was previously described in ref. 55. The calculation of the magnetic properties—isothermal magnetizations and magnetic susceptibilities—using these wavefunctions and energies were

Fig. 1 Fe(CH3)2, Fe(NH2)2, and Fe(OH)2 DFT-optimized model complexes with D3d, D2h, and C2h geometries employed in the analysis of the FeII–ligand chemical bond and the pseudo Jahn–Teller activity of the d6 conﬁguration of FeII; Orange, gray, blue, red and cyan spheres represent Fe, C, N, O and H atoms, respectively.

This journal is ª The Royal Society of Chemistry 2013

Chemical Science detailed in a recent publication.46 In order to study vibronic coupling eﬀects, starting with complex 2, possessing trigonal symmetry and the pseudo Jahn–Teller eﬀect in complexes 1 and 3–7, we employed the truncated model complexes Fe(CH3)2, Fe(NH2)2 and Fe(OH)2 (see Fig. 1).

2.2

Ligand eld considerations 5

The E ground state of FeC2 (complex 2, accounting for the trigonal symmetry due to the next-nearest neighbors) is described by a total spin S ¼ 2 arising from two singly occupied orbitals e(dx2y2) or e(dxy) in addition to the half-lled d5 shell. These states give rise to ML ¼ 2 eigenfunctions of the angular ^z (eqn (1)). momentum operator L pﬃﬃﬃ 5 E; 2 ¼ 1= 2 5 E; dx2 y2 i5 E; dxy (1) Note that the states r5E,2i and r5E,2i cannot mix under the ^x and L ^y since ML changes by 1 unit of angular action of L ^x and L ^y. Mixing of these states with the momentum through L higher-lying 5E(dxz,yz)1 (ML ¼ 1), levels is possible. However, the latter are much higher in energy and will be neglected here. The eﬀects of these states on the magnetic properties will be discussed in Section 3.2.3 and 3.3. In this approximation, the spin–orbit ^ SOC assumes the form of eqn (2). coupling (SOC) operator H H^ SOC ¼ (z/4)L^zSˆz

(2)

^ SOC is represented by a diagonal 10 Within the rMS,MLi basis, H 10 matrix with elements (z/4)MSML (MS ¼ 0, 1, 2 and ML ¼ 2).58–61 The parameter z is the eﬀective one-electron SOC ‘constant’ for FeII (see ref. 17 and 62 for a detailed discussion). The energetic eﬀect of low-symmetry perturbations on the 5 E(dx2y2) and 5E(dxy) sublevels can be described in terms of two parameters d1 and d2 accounting for the splitting and mixing of 5 5 E dx2 y2 E dxy " # (3) d1 d2 H^ LF ¼ d2 d1 j2i " 5

5

j2i

0

d1 id2

d1 þ d2

0

#

(4)

these states as given by eqn (3). Following eqn (1), these sublevels can be transformed into a ML ¼ 2 basis (eqn (4)). The physical origin of d1 and d2 will be subject to a thorough ^ SOC + analysis in Sections 3.2.3 and 3.3. The Hamiltonian H ^ Z (H ^ Z ¼ the Zeeman operator) represented in the rML ¼ ^ LF + H H 2, MS ¼ 2, 1,0i basis, as well as energy and g-tensor expressions (normalized to a m ¼ 1/2 pseudo spin)25 are given in the ESI.† The [Fe(tpaR)] single-molecule magnets from ref. 22 and 23 possess trigonally elongated geometries and a 5 E(dxz,yz)1 ground state. Here, SOC leads to two lowest magnetic levels A1 and A2 which are split by the trigonal symmetry. Being an equal mixture of total angular momenta with MJ ¼ +3 and MJ ¼ 3, these states carry no magnetic moments. The Chem. Sci., 2013, 4, 139–156 | 141

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

complexes of the present study are completely diﬀerent. The ground state for linear complexes FeX2 is 5E(dxy,dx2y2)1 (complex 2, FeC2, can be ascribed as a trigonally compressed one), which under the action of SOC leads to a E(MJ ¼ 4) magnetic ground state. For both types of FeII-based singlemolecule magnets, and within the given approximation, pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ geometric distortions described by d ¼ d1 2 þ d2 2 s 0 do not cause a splitting of the MJ(MS s 0) pairs, leaving A1 and A2 in the former type of complexes accidentally degenerate. Quite diﬀerently, MJ levels with MS ¼ 0 undergo a rst-order splitting (2d) depending p onﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ the magnitude of the distortion (in ﬃ energetic sense, d ¼ d1 2 þ d2 2 s 0) but not on its direction (i.e., on 4, tg4 ¼ d2/d1). From eqn (1)–(4), the origin of the magnetic anisotropy arises; without oﬀ-axial distortions ﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðd ¼ d1 2 þ d2 2 ¼ 0Þ there is a 1 : 1 mixing between the |dx2y2i1 and |dxyi1 sublevels of the 5E term by SOC, and this leads to the addition of an orbital angular momentum of 2 mB to the net spin S ¼ 2 moment (4 mB). Focusing on the |MJ ¼ 4i ground state magnetic pair, an Ising-type anisotropy with gz ¼ 12 and gx,y ¼ 0 (d z) is obtained. In the limiting case of very large distortions (d [ z), the latter reduces to the spin-only values of gz ¼ gx ¼ gy ¼ 8. 2.3

The 5E53 Renner–Teller eﬀect

Unlike bent complex 6 and linear complex 7, the pseudolinear FeX2 cores in 1–5 possess inversion symmetry. Therefore, no linear vibronic coupling with the oﬀ-centric normal modes, 3, which serve to distort the linear geometry to a bent structure is possible. The energy lowering and energy splitting of the 5 E(dx2y2dxy)1 ground state of the FeII complexes due to Renner– Teller (RT) vibronic coupling is described by eqn (5),63–69 in which the nuclear coordinates Qx and Qy are components of the 3 mode (eqn (6)), r is the RT radius (eqn (7)), and 4 (eqn (8)) denes the direction of the distortion. 2 g 2 1 E ¼ K3 Qx 2 þ Qy 2 þ j Qx 2 þ Qy 2 Qx 2 þ Qy 2 2 2 1 2 4 ¼ ðK3 gÞr þ jr 2

Qx ¼ rcos 4; Qy ¼ rsin 4 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r ¼ Qx 2 þ Qy 2

(7)

tg4 ¼ Qy/Qx ¼ d2/d1

(8)

The parameters K3 and j describe the eﬀect of the harmonicity and anharmonicity, respectively (i.e., two terms due to forces which tend to preserve the linear geometry). The g-term quanties the vibronic force that leads to distortions and, accordingly to a splitting (g(Qx2 + Qy2)) of the 5E(dx2y2,dxy)1 ground state (eqn (5)). Depending on whether K3 > g or K3 < g, two diﬀerent situations are encountered (see Fig. 2). In the rst case, no new minima in the adiabatic ground state potential energy surface (APES) arise; however, the adiabatic approximation is violated by the vibronic mixing (via a term gQxQy) between the two sublevels. The other extreme, K3 < g, leads to a negative curvature for the lower surface, and therefore to dynamical instability. As a consequence, new minima on the APES corresponding to bent structures arise. Energy expressions, derived in the ESI,† allow us to relate the parameters K3, j, and g with the geometry of the minimum of the adiabatic ground state potential surface (APES) (rmin), the Renner–Teller stabilization energy ERT, and the energy of the vertical Franck–Condon transition EFC from the lower to the upper sheet of the APES (at the position of the minima) in terms of g, K3 and j. In turn, using these expressions g–K3 and j have been deduced from DFT values of rmin and ERT, obtained from a truncated FeC2 model complex (see Fig. 1). An estimate for K3 ¼ h- u3 is obtained using he corresponding Zn(CH3)2 analog, which lacks RT-activity. This leads to the parameters h- u3 ¼ 131 cm1, g ¼ 461 cm1, and j ¼ 8.2 cm1. Energy eigenvalues and eigenfunctions of vibronic levels were calculated using a Hamiltonian of the form: ^ vib + H ^ SOC + H ^ RT + H ^Z H^ ¼ H

(5)

(6)

(9)

^ vib including the with the harmonic vibrational Hamiltonian H ^ ^ RT, and H ^ Z, potential and kinetic energy terms and H SOC, H

Fig. 2 Variable adiabatic potential energy surface of a FeIIX2 complex with a doubly degenerate 5D ground state with respect to the oﬀ-centric displacement Qx in the case of the 5D5p Renner–Teller eﬀect: weak coupling – term splitting without instability (left); strong coupling – dynamic instability; nuclear probability distributions h|j|2i are shown with dotted lines.

142 | Chem. Sci., 2013, 4, 139–156

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

Chemical Science

representing the spin–orbit coupling, Renner–Teller, and Zeeman energy operators, respectively. The Hamiltonian of eqn (9) has been set up in the basis rJi of the products of electronic wavefunctions rfii ¼ rML ¼ 2, MS ¼ 2, 1, 0i, i ¼ 1 : 10 and 0 0 harmonic vibrational |cj(Qxi$|ck(Qyi wavefunctions up to level nvib (see ESI† for details). Isothermal magnetic susceptibilities and magnetizations were calculated employing the representa^ Z in the basis rJi and making explicit use of the tion of H calculated eigenvectors following procedures outlined previously.46

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

2.4

Ligand eld analysis of the ab initio results

Ab initio results were analyzed by mapping the ab initio multireference wavefunctions and energies onto ligand eld theory in the manner developed in detail in ref. 70. In this treatment, the LF Hamiltonian is viewed as an eﬀective Hamiltonian that acts on the subspace of states originating from a given dnconguration of a transition metal subject to perturbations from surrounding ligands. For an FeII center without including SOC, the d6 conguration spans 5, 45 and 50 electronic states with total spins of S ¼ 2, 1, and 0, respectively. The LF Hamiltonian within this basis is expressed in terms of a LF 5 5 matrix for one d-electron and atomic like parameters of interelectronic repulsion B and C. The energies of the ve S ¼ 2 states for FeII do not depend on the parameters B and C, and the LF matrix for the ve S ¼ 2 levels can be identied with the 5 5 LF matrix for one d-electron. From the possible parameterization oﬀered by the LFT, the angular overlap model (AOM) nds most favor among chemists.71–73 This model expresses the matrix elements of the 5 5 LF matrix in terms of parameters dened for well-aligned d-orbitals of s- and p-type, el (l ¼ s, pc, ps) multiplied by factors Flu(ql, 4l, jl) that depend solely on the angular geometry of the ligands (l, described by the Euler angles ql, 4l, jl). AOM energy expressions for a FeX2 complex with C2v symmetry (with a choice of Cartesian axes as shown in Fig. 3) have been derived and listed in the ESI.† The parameters es, epc, and eps quantify the energy destabilization of the FeII d-orbitals due to their negative overlap with the corresponding wellaligned ligand orbitals of s- and p-type (see Fig. 4), where

Fig. 4 Interactions approximating the FeII–ligand bond in FeN2 complexes 1, 3– 4, 6, and 7 (upper), FeO2 complex 5 (middle), and FeC2 complex 2 (lower), and their angular overlap model parameterizations.

anisotropy of the interactions of p-type, epc and eps, is taken into account (see Fig. 3 and 4 for the denition of the angle q and the AOM parameters, respectively). For a linear FeX2 complex (q ¼ 0 ) with dominating ligand donor functions of es > epc ¼ eps ¼ ep > 0, all parameters being positive in this case, the orbital energy order d(dx2y2, xy) < p(dxz,yz) < s(dz2) results:

e d dx2 y2 ;xy ¼ 0

(10) e p dxz;yz ¼ 2ep e½sðdz2 Þ ¼ 2es AOM parameters are traditionally deduced from a t to electronic d–d transitions observed in absorption and emission spectra of transition metal complexes. This procedure is oen (although not always) challenging, because the number of parameters is too large to allow for a unique determination. Recently, a procedure was proposed allowing one to deduce the LF parameters from ab initio calculations,70 which can be summarized as follows. First, focusing on the S ¼ 2 states, the 5 5 CI matrix in the basis of the Slater Determinants (SDs) built up from the metal-3d based molecular (CASSCF) orbitals is calculated. Focusing on SDs with MS ¼ S ¼ 2, we note that each single SD is a spin eigenfunction (i.e., SDs and conguration state functions (CSFs) are identical in this case). With the output of the electronic structure program, the CASSCF eigenvalues (EICASSCF) and eigenfunctions CCASSCF(1 : 5, I) (I ¼ 1 : 5) are directly available. Let us denote the diagonal matrix constructed from EICASSCF with LCASSCF(EICASSCF,I ¼ 1 : 5). We then deduce the LF matrix HLFT ¼ {HLFT IJ ,I,J ¼ 1 : 5} using the transformation: † HLFT CASSCF ¼ CCASSCFLCASSCFCCASSCF

Fig. 3 1–7.

Cartesian axes choice and geometrical parameters for the FeX2 core in

This journal is ª The Royal Society of Chemistry 2013

(11)

Dynamic correlation eﬀects are introduced via diagonal corrections to LCASSCF as provided by second-order many-body perturbation theory in form of the NEVPT2 method (DLNEVPT2, eqn (13)). The AOM parameters (pl) are then obtained by a leastsquares t based on eqn (14), where the matrices HAOM and HLFT NEVPT2 have been transformed into the traceless forms HAOM (pl) and HLFT b NEVPT2,b, respectively. Chem. Sci., 2013, 4, 139–156 | 143

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

† HLET NEVPT2 ¼ CCASSCFLNEVPT2CCASSCF

(12)

LNEVPT2 ¼ LCASSCF + DLNEVPT2

(13)

(pl) ¼ HLFT HAOM b NEVPT2,b

(14)

Adopting the one-electron parameters without changes, the parameters B and C were obtained from the computed energies of the spin–forbidden transitions, which, in the present case, are the transitions from the 5E ground state to the triplet ligand eld excited states. Finally, using es, ep, B, and C and switching on SOC, we x the value of z from the computed energies of the 5 E ground state SOC split sublevels. These calculations were performed through an interface between the ORCA program and the well-established ligand eld program package AOMX.74

3

Results and discussion

1, 3, 4, 6, and 7, with N-amido donors, there is a plane dened by N and the directly connected two atoms X forming N–X bonds; here X represents C and Si (1), C and H (3, 4, and 6), or two C atoms (7). As the FeII center is located in the same plane as the N(sp2)-donor atoms and their nearest neighbors, there is a well-dened direction for the p-interactions between FeII center (according to Fig. 4, the appropriate iron orbital is dyz) and the amido p-electron pair of the same symmetry (dened here as ps type in AOM). Since the Fe–N bond can be considered as weaker than the N–X bonds, we assign the local Fe–ligand bond a pseudosymmetry of C2v. Finally, in complex 5 there are two donor lone-pairs; one of these pairs, similar to Fe–N, has the symmetry appropriate for ps-type overlap with the out-ofthe Fe–O–C plane dyz orbital, while the other pair (located within the Fe–O–C plane) is available for pc-type overlap with the metal dxz orbital. This arrangement denes a local Cs pseudosymmetry.

3.1 Chemical bonding and vibronic activity of twocoordinate complexes of FeII It follows from X-ray data that the FeX2 cores in complexes 1–5 and 7 are linear. However, due to the nearest and next-nearest neighboring atoms of the FeII center, the electron density distribution deviates from idealized DNh symmetry. It has been shown that the second coordination sphere aﬀects metal– ligand bonding and results in dramatic changes to the color and magnetism of transition metals in solid matrices.75 Of immediate interest is the extent to which the next-nearest atoms in the coordination sphere of the FeII center aﬀect the magnetic properties of complexes 1–7. Depending on the number of strong bonds formed by the donor atoms C, N, or O (see Fig. 4), these complexes can be subdivided into three classes. With the C donor involved in three strong bonds to neighboring Si atoms, and neglecting hyperconjugation, there are no ligand orbitals available for FeII–C interactions of p-type in complex 2. The local symmetry around the Fe–C bond is C3v. In complexes

Table 1

Fig. 5 Molecular orbitals (DFT, PBE-functional) with contribution from the 3dorbitals of FeII as exempliﬁed using the Fe(NH2)2 model complex. From bottom to top, the s-interactions (left) are bonding and weakly and strongly antibonding, while the ps-interactions (right) are bonding and antibonding.

Molecular orbital energies and compositions characterizing the participation of the FeII orbitals in the bondinga

Fe(CH3)2

Fe(NH2)2

Fe(OH)2

s-type orbitals 7.45(bd): 11(4s) + 29(3dz2) [2] 5.40(weakly ab): 20(4s) + 50(3dz2) + 16(3dx2y2) [2] 5.37(nb): 4(4s) + 10(3dz2) + 10(3dxz) + 73(3dx2y2) [1] 0.32(ab): 47(4s) + 13(3dz2) [0]

s–pc type orbitals 9.55(bd): 8(4s) + 20(3dz2) [2] 4.91(weakly ab): 16(4s) + 48(3dz2) + 27(3dx2y2) [1] 4.06(nb): 8(4s) + 16(3dz2) + 72(3dx2y2) [1] 0.56(ab): 42(4s) + 15(3dz2) [0]

s–pc type orbitals 11.86(bd): 5(4s) + 12(3dz2) [2] 7.84(bd): 1(4s) + 6(3dz2) 5(4s) + 13(3dxz) [2]

p-type orbitals 5.69(nb): 86(3dxz) + 10(3dx2y2) [1] 5.65(nb): 95(3dyz) [1] d-type orbital 4.60(nb): 99(3dxy) [2]

ps-type orbitals 5.94(bd): 37(3dyz) [2] 3.58(ab): 66(3dyz) [1] pc-type orbital 4.88(nb): 96(3dxz) [1] d-type orbital 4.99(nb): 100(3dxy) [1]

5.24(weakly ab): 17(4s) + 57(3dz2) + 16(3dxz) + 3(3dx2y2) [1] 4.72(weakly ab): 7(4s) + 6(3dz2) + 71(3dxz) + 2(3dx2y2) [1] 4.33(nb): 2(4s) + 3(3dz2) + 95(3dx2y2) [2] 1.08(ab): 49(4s) + 17(3dz2) [0] ps-type orbitals 7.33(bd): 24(3dyz) [2] 4.38(ab): 78(3dyz) [1] d-type orbital 5.14(nb): 100(3dxy) [1]

a bd – bonding; ab – antibonding; nb – non-bonding; quasi restricted orbitals from DFT optimized model complexes (see ESI† for more details regarding these calculations); orbital electron occupation numbers are given in square brackets.

144 | Chem. Sci., 2013, 4, 139–156

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article

Chemical Science

Molecular orbital energies and Fe orbital percentages, deduced from quasi restricted DFT calculations performed on truncated Fe(CH3)2, Fe(NH2)2 and Fe(OH)2 model complexes (see Fig. 1) are listed in Table 1. Focusing on Fe(CH3)2, we note that, as expected, the Fe–C bonding is solely governed by strong Fe–C s-interactions, with the main participation coming from Fe 4s and 3dz2 orbitals; other orbitals (dxz, dyz, and dxy) are nonbonding due to a lack of ligand orbitals of appropriate symmetry. The interaction of the metal centered 3dz2 and 4s orbitals with the ligands gives rise to bonding, antibonding, and weakly antibonding MOs, as illustrated for Fe(NH2)2 at the le of Fig. 5. It is the intermixing of 4s into the nominally 3dz2 Fe-based orbital (as strong as 20% for Fe(CH3)2 and 16% for Fe(NH2)2) which converts this orbital from strongly antibonding (typical for octahedral complexes) to weakly antibonding in the FeX2 complexes 1–7. As will be shown below, this has an important eﬀect on the magnetic properties. In contrast to Fe(CH3)2, the out-of-plane type of p-bonding (ps) is essential in Fe(NH2)2 and Fe(OH)2. Here, a strong mixing between the FeII(dyz) and the corresponding ligand functions takes place, giving rise to the bonding and antibonding MOs, as illustrated for Fe(NH2)2 at the right in Fig. 5. The Cs symmetry of the Fe–O–H moiety leads to a mixing of the metal-based orbitals dz2, dxz, and dx2y2 (all behave totally symmetric with respect to the Fe–O–H symmetry plane). In a strictly linear complex, such as Cl–Fe–Cl, these orbitals would have s, pc, and dc character, respectively (see eqn (10)). However, based on the dz2, dxz, and dx2y2 FeII orbital percentages (57%, 71%, and 95% in the MOs with energies 5.24, 4.72 and 4.33 eV, respectively) the assignment given by the AOM (eqn (10)) is roughly correct. Linear (DNh) FeX2 complexes with a 5D(dx2y2,xy) ground state are intrinsically unstable with respect to geometric distortions since they are Renner–Teller active. Thus, bending of these complexes can cause the strictly non-bonding dx2y2,xy orbitals to become involved in bonding/antibonding interactions due to mixing of these orbitals with the p(dxz, yz) and s(dz2) orbitals and their ligands counterparts. The reduction in total energy is the driving force for such distortions. Calculating geometries from rst principles for such complexes is still far from trivial. First, at the point of orbital degeneracy and close to it, DFT is not applicable, while CASSCF is usually not accurate enough and many body perturbation approaches, such as NEVPT2, suﬀer from a lack of availability of analytic gradients, at least for larger molecules. Second, a ground state APES with two minima at distorted geometries is stationary at the point of degeneracy,

˚ bond angles in ), energy Table 2 Geometrical parameters (bond distances in A, stabilizations, Renner–Teller Radii rmin and C–M–C bending mode vibrational energies for Zn(CH3)2, Mn(CH3)2, and Fe(CH3)2 model complexes from DFT geometry optimizations

Zn(CH3)2 Mn(CH3)2 Fe(CH3)2

R

2(90 q)

E

rmin

n[d(X–Fe–X)] (cm1)

1.952 2.064 2.006

180 158.3 144.5

0 233 964

0 1.80 2.50

136 124 134

This journal is ª The Royal Society of Chemistry 2013

implying that the energy gradient at that point is zero. Therefore, while keeping to DFT, use of a distorted structure as the starting geometry in a geometry optimization is advisable. Third, the APES is highly anharmonic, implying the requirement of higher-order polynomials (up to order 8 for the cases studied below) in the Herzberg–Teller series66 expansion to model the energy of the 5D(dx2y2,xy) APES. DFT geometry optimizations of FeX2 (X ¼ CH3, NH2, and OH) starting from bent geometries resulted in a bent structure for Fe(CH3)2 with an X–Fe–X angle of 144.5 , but resulted in linear structures for Fe(NH2)2 and Fe(OH)2 (see Table 2). Based on a normal mode analysis, all geometrically optimized structures with linear FeX2 cores were calculated to be stable with respect to X–Fe–X bending. For the reasons stated previously (breakdown of the adiabatic approximation for closely-lying electronic levels), numerical values of the harmonic X–Fe–X frequencies are questionable. However, based on the very low values of these frequencies (see Table 2), they are still strongly indicative of so mode behavior. The quantication of the eﬀect of the latter on the magnetic properties will be analyzed below (see Section 3.2.2). A scan of the ground state energy versus the X–Fe–X angle for Fe(CH3)2 and the analogous Mn(CH3)2 and Zn(CH3)2 complexes with half lled (d5) and closed shell (d10) electronic congurations for the MII center, respectively, is shown in Fig. 6. To avoid the point of degeneracy, in these calculations X–M–X angles higher than 170 were excluded. A least-squares t to the data with a polynomial of degree 8 (solid lines in Fig. 6) allows one to deduce the energy of the linear geometry via interpolation. Remarkably, not only Fe(CH3)2 but also Mn(CH3)2 is stabilized by bending. It is interesting to note, that [FeCl2]+ (which is isoelectronic with Mn(CH3)2) is

Fig. 6 Adiabatic potential energy (in cm1) surfaces (APES) for M(CH3)2 (M ¼ Mn, Fe, Zn) model complexes, illustrating dynamical instabilities in the cases of Mn(CH3)2 (3d–4p pseudo Jahn–Teller coupling) and Fe(CH3)2 (3d–4p pseudo Jahn–Teller coupling superimposed by a (stronger) 5E53 Renner–Teller eﬀect). DFT optimized M–ligand bond distances are almost unchanged along the distortion path and have been ﬁxed at their values at the minimum of the APES (see Table 2). The APES has been constructed by varying the angle q (see Fig. 3 for its deﬁnition) between 45 and 80 in steps. Solid lines reproduce the data in terms of a polynomial of the degree 8: P(1)$Q8 + P(3)$Q6 + P(5)$Q4 + P(7)$Q2 + P(9) with the following values of the coeﬃcients P(1), P(3), P(5), P(7), and P(9): 0.0288, 1.7513, 43.0557, 362.0133, and 953 for Fe(CH3)2; 0.0181, 1.1037, 27.7868, 150.9680, and 232.8404 for Mn(CH3)2; 0.0514, 0.6800, 1.0285, 459.3716, and 234.2324 for Zn(CH3)2. Here, Q is expressed by the variable angle q at ﬁxed values of the metal–ligand bond distance R (from Table 2) according to Q ¼ 2R(90 q)(p/180).

Chem. Sci., 2013, 4, 139–156 | 145

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

calculated by DFT to be distorted as well, with an X–Fe–X angle of 132.2 and with an appreciably large stabilization energy of 1250 cm1. The origin of this eﬀect is found in the diﬀerent roles played by the 4px,y valence orbitals of FeII in the linear and bent congurations, respectively (see ESI†). Being non-bonding (due to their high energy separations from the ligand orbitals) and of diﬀerent parity (compared to 3d), the 4px,y AOs are essentially non-bonding in linear Mn(CH3)2. As illustrated in the ESI,† bending leads to a considerable mixing of 4px,y into 3dyz,xz, because both orbitals transform under the same irreducible representation in C2v. This mixing, or partial hybridization, leads to an increase of both s- and, to a lesser extent, ptype metal–ligand overlap. The eﬀect can be considered to be analogous to 3d–4s mixing for linear geometries but is energetically less pronounced. The extra electron in the dx2y2,xy orbital pair leads to an enhancement of the distortion (rmin) and an additional energy stabilization (E) as the comparison ˚ E ¼ 233 cm1) and between Mn(CH3)2 (rmin ¼ 1.80 A, ˚ E ¼ 964 cm1) shows (see Fig. 6 and Fe(CH3)2 (rmin ¼ 2.50 A, Table 2). Using data in Table 2, parameters of the vibronic coupling model were derived as specied in Section 2.3.

3.2

Electronic (vibronic) levels and magnetic properties

3.2.1 THE STATIC MODEL. The d6 conguration of the FeII centers in complexes 1–7 gives rise to 5 quintet states with NEVPT2 energies computed on the basis of the crystal structures listed in Table 3. The ground state of all complexes is a quintet 5E state with an energy that is lower by 15 200–20 600 cm1 than that of the lowest triplet state. The electronic absorption spectrum of 1 in 2-methyltetrahydrofuran consists of a broad asymmetric band centered at 8500 cm1 (see ESI†). Its simulation with two Gaussian envelopes led to the identication of the energies of the two expected d–d transitions centered at 7700 and 9400 cm1, respectively. These numbers compare well with the calculated CASSCF/

NEVPT2 transition energies (6936 and 10 062 cm1). We accordingly assign these as electronic transitions from 5 E(dx2y2,xy)1 to 5A1(dz2)1 and the 5E(dyz)1 split component of the 5 E(dyz,xz)1 state, with the lower energy transitions assigned to the 5E(dxz1) component and the even lower transitions within the 5E(dx2y2,xy)1 SOC sublevels manifold lying outside the spectrally accessible energy range. Deviations from axial symmetry (see Section 3.1) lead to a non-relativistic ground state splitting that is lowest for 2 (92 cm1) and increases from 4 (381 cm1) to 7 (766 cm1) and 6 (1246 cm1). The 5E ground state splitting for complexes 1, 3, and 5 (164, 241, and 222 cm1, respectively) are intermediate between those of 2 and 4 and thus lie outside the observed trend. This behavior will be analyzed below. The magnetic sublevels (classied according to the D3 symmetry encountered in complex 2) arising from the 5E ground state aer SOC are also included in Table 3. The ordering of these sublevels and their relative energy separations closely follows the energy expressions derived from a simplied treatment (see ESI†) in which only the in-state 5E SOC is considered. This behavior reects the dominant role of SOC, which widely suppresses low-symmetry splitting of all sublevels pairs with non-zero ML. In particular, splitting of the ground state magnetic sublevels |ML ¼ +2, MS ¼ +2i and |ML ¼ 2, MS ¼ 2i, through mixing with the topmost state |ML ¼ 2, MS ¼ +2i and |ML ¼ +2, MS ¼ 2i, respectively, is prevented by the large energy gap (2z z 800 cm1) between the two sublevels. This splitting is more pronounced for the rst excited states |ML ¼ +2, MS ¼ +1i and |ML ¼ 2, MS ¼ 1i, which interact with their respective |ML ¼ 2, MS ¼ +1i and |ML ¼ +2, MS ¼ 1i counterparts, because the former states are separated by a twofold smaller energy (z z 400 cm1). Being not aﬀected by SOC, the state E |ML ¼ 2, MS ¼ 0i is the only one that is strongly inuenced by oﬀ-axial distortions; its splitting is identical to that of non-relativistic 5E ground state (see Table 3). Using all of the SOC split sublevels of 5E ground state parentage and their associated wavefunctions, magnetizations

Table 3 Energies (in cm1) of S ¼ 2 states, of the lowest excited S ¼ 1 state (3A), and of the spin–orbit split components of the lowest 5E (D3 symmetry notations) from NEVPT2 calculations of linear FeX2 complexes with geometries from X-ray diﬀraction data and accounting for the complete set of the 5 quintet and 45 triplet electronic statesa

Electronic statea

1

2

3

4

5

6

7

5 E(dxy)1 (dx2y2)1 5 E(dxz)1 (dyz)1 5 A(dz2)1 3 A E(1)

0 164 3726 10 468 [9400] 7068 [7700] 18 023 0 0.002 189.8 190.4 322.8 485.8 612.8 625.0 810.1 810.3

0 92 4760 4799 5087 20 622 0 0.001 195.2 195.3 353.0 444.6 602.0 603.8 799.7 800.0

0 241 2080 8156 9190 14 944 0 0.013 176.4 179.8 286.6 529.1 632.0 646.6 822.0 822.5

0 381 2372 8057 9623 14 826 0 0.022 158.4 163.2 242.7 624.6 704.4 710.1 870.4 870.7

0 222 5004 7124 11 002 16 813 0 0.004 183.9 185.6 300.9 521.4 632.8 641.5 820.4 820.5

0 1246 8829 2409 9907 20 176 0 0.078 78.1 84.9 111.2 1347.5 1373.2 1384.4 1464.7 1464.8

0 766 6820 7649 8409 15 947 0 0.020 122.3 123.3 172.2 937.6 985.7 986.8 1106.7 1106.8

A1,A2(1) E(2) E(3) A1,A2(2) a

Experimental transition energies from near-IR d–d spectra of 1 are listed in square brackets.

146 | Chem. Sci., 2013, 4, 139–156

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article

Chemical Science

Fig. 7 Upper: experimental (blue squares) and calculated (NEVPT2, red circles) magnetic susceptibility data for complex 1 in the temperature range from 2 to 300 K under a static applied dc ﬁeld of 1000 Oe. Lower: experimental (squares) and calculated (NEVPT2, red circles) isothermal magnetization M vs. H/T for complex 1.

(M) and susceptibilities (cT) were calculated for 1–6. NEVPT2 values for cT and M for complexes 1 and 2 are both in good agreement with experimental data (see Fig. 7 and ESI†). The direct-current magnetization measurement at 1.85 K of the same crystalline sample as used for the M¨ ossbauer study28 yielded Mz ¼ 5.82 mB, which is very close to the NEVPT2 result (5.98 mB) for a sample of crystallites fully aligned with the applied magnetic eld. The experimental data given in ref. 55 are also in good agreement with the NEVPT2 result; however, here the NEVPT2 results have been converted to a powder average. The error for the data in ref. 28 is less than 3% away 0 from the maximal achievable magnetic moment of 6 mB (gMJ, 0 g ¼ 2, MJ ¼ 3). The situation changes for complexes 3–5 and 6. Here, the comparison between theory and experiment for cT and M (see

Table 4 and ESI†) shows that the calculated values are systematically larger than the experimental ones. The same complexes 3–5 display a drastic reduction (by as much as two to three orders of magnitude) in their relaxation times, as compared to 1 and 2.55 One could speculate that spin–orbit coupling (z), which is usually slightly overestimated in post Hartree–Fock calculations,46 might be responsible for the observed deviations. However, using empirically reduced values of z (accounting for the relativistic nephelauxetic eﬀect17 in the crudest possible way with an orbital reduction factor k) does not alleviate the problems. Thus, focusing on complex 3, both cT and M can only be brought into agreement with experiment by using an anomalously low orbital reduction factor k ¼ 0.6 (see ESI†). Hence, the deviations between theory and experiment must have a diﬀerent origin, as will be discussed in detail below. 3.2.2 DYNAMIC VIBRONIC COUPLING. From the preceding analysis it becomes clear that a model based on a static distortion is not able to account for the anomalously reduced magnetic moments reected in the measured susceptibilities and magnetizations of complexes 3–6. As detailed in Section 2.3, the 5E electronic state is vibronically unstable. In order to study the eﬀect of this instability on the magnetic properties, the energies and wavefunctions of the vibronic levels for the instate 5E53 vibronic coupling problem were computed utilizing the set of vibronic parameters K3 ¼ h- u, g and j adjusted to the ground state APES of Fe(CH3)2 (see Section 2.3). Variation of the vibronic coupling strength is accounted for in terms of the dimensionless parameter (f) which scales the Renner–Teller vibronic coupling constant g as well as the vibronic anharmonicity parameter j (f$g and f$j, respectively), while keeping the harmonic frequency of the 3 X–Fe–X bending mode (K3 ¼ h- u ¼ 131 cm1) unchanged. By increasing the value of f from 0 (static limit) to 1 (the strong coupling limit adjusted to the energy landscape pertaining to Fe(CH3)2), the eﬀect of the vibronic coupling strength on cT and M was systematically traced. Vibronic energy levels as functions of the parameters f are plotted in Fig. 8. Points at the le hand side of the diagram (f ¼ 0) correspond to energies of vibronic levels represented by basis functions built up as simple products of electronic |MJ ¼ ML + 0 0 MSi and vibrational |ck(Qx)cl(Qy)i parts, with energies of the uncoupled electron and nuclear motions given by eqn (15) (see ESI† for a visualization of the energy levels in this limiting case).

Table 4 Experimental and calculated (using molecular geometries from X-ray data, NEVPT2 results) values of the magnetic susceptibility (cT) and the isothermal magnetization (M) at 300 K and 2 K for complexes 1–6 (static model) and values of the vibronic coupling strength parameter f of a dynamic Renner–Teller model utilized to ﬁt the magnetic susceptibility data

Complex

1 Exp(calc.)

2 Exp(calc.)

3 Exp(calc.)

4 Exp(calc.)

5 Exp(calc.)

6 Exp(calc.)

(cT)300K f300K (cT)2K f2K MHTLFa MLTHFb

4.45(4.76) 0c 4.17(4.22) 0c 2.47(2.48) 3.00(3.00)

4.78(4.82) 0c 4.33(4.30) 0c 1.50(1.42) 3.24(3.04)

3.35(4.35) 0.133 3.73(4.80) 0.082 1.23(1.44) 2.74(3.10)

3.37(4.76) 0.132 2.88(4.30) 0.099 0.96(1.43) 2.14(3.11)

3.19(4.87) 0.162 2.87(4.46) 0.099 0.92(1.47) 2.06(3.15)

2.87(3.99) 2.03(3.44) 0.74(1.17) 1.93(2.88)

a MHTLF (high-temperature low-eld): T ¼ 5 K, H ¼ 1 T. b MLTHF (low-temperature high-eld): T ¼ 1.8 K, H ¼ 7 T. c Marks the appearance of a static limit corresponding to a value of f close to 0.

This journal is ª The Royal Society of Chemistry 2013

Chem. Sci., 2013, 4, 139–156 | 147

View Article Online

Chemical Science

Edge Article

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

decrease in the orbital contributions to the net magnetic moment and a concomitant change in the magnetic properties. From the energies and term assignments of the ve lowest magnetic levels (see Fig. 8, lower), we deduce that the level ordering (E < E < A1) in a dynamic Renner–Teller regime is completely diﬀerent than the one that applies in the static limit. In both cases the lowest sublevels remain doubly degenerate. Thus, the main diﬀerence is that the electronic degeneracy gives way to a vibronic one. One can qualitatively understand this behavior jML ¼ 2; MS ¼ 2; c0 ðQÞi jML ¼ H2; MS ¼ 2; c2 ðQÞi 3 2 1 1 pﬃﬃﬃ fg 7 6 2 hu3 z 7 2 2 6 7 6 7 6 7 4 1 5 pﬃﬃﬃ fg hu3 þ z 5 2 2 2 (16)

Fig. 8 Upper: vibronic energy levels from calculations on a Fe(CH3)2 model complex in the energy range below 900 cm1 versus the vibronic coupling strength parameter f scaling the vibronic parameters g ¼ 461 cm1 and j ¼ 8.19 cm1 of eqn (5). Lower: low energy range of the ﬁve lowest vibronic states responsible for the magnetic behavior (h- u3 ¼ 131 cm1). The ground state E(1) and the lowest excited state E(2) responsible for the energy barrier Ueﬀ of the Orbach relaxation mechanism are depicted in red.

through a two state model by restricting attention to a single interacting mode Q.63 Starting from the weak vibronic coupling limit (small f), the ground state is represented by |ML ¼ +2, MS ¼ +2, co(Q0 )i and |ML ¼ 2, MS ¼ 2, co(Q0 )i. These wavefunctions can only vibronically mix with |ML ¼ 2, MS ¼ +2, c2(Q0 )i and |ML ¼ +2, MS ¼ 2, c2(Q0 )i, respectively, as given by the matrix in eqn (16); here, co(Q0 )and c2(Q0 ) are the ground state and second excited state harmonic oscillator wavefunctions, respectively. For small f the separation between the two states (2(2 + h- u)) is large, while the mixing is small pﬃﬃﬃ (½ð1=2 2Þ fg 2ðz þ h- uÞ, Fig. 2, le). Thus, there are negligible contributions of the ML ¼ H2 orbital moments of opposite sign to the ground state magnetic pair ML ¼ 2. The probability distribution for the nuclear motion is close to Gaussian type |co(Q0 )|2 (see Fig. 2, le) with a maximum at the undistorted (linear) nuclear conguration. Let us now assume the other extreme: the strong Renner–Teller coupling limit of f ¼ 1. Here, there is nearly 1 : 1 mixing between the orbital moments ML ¼ +2 and ML ¼ 2, which are now better approximated by the |dx2y21i and |dxy1i spatial components and ground vibronic state described by two ground state 0 harmonic oscillator wavefunctions, displaced by 2Qo in congurational space relative to the undistorted geometry,

Fig. 9 Dependence of the z-components of the g-tensor in the lowest ﬁve thermally accessible magnetic states on the vibronic coupling strength parameter f.

E(MJ ¼ ML + MS,k, l) ¼ (z/4)MLMS + (k + l + 1)h- u

(15)

A mixing of these wavefunctions for non-zero f leads to the opening of a gap between the ve lowest levels and the other excited states (see Fig. 8, upper) and this gap increases with f. Thus, at values of f close to 0.1, a discontinuity in the spectrum of the magnetic excitations is predicted to occur. As illustrated by the dependence of the z-components of the g-tensor (see Fig. 9), the opening of the gap leads to a dramatic

148 | Chem. Sci., 2013, 4, 139–156

Fig. 10 Adiabatic potential energy surface in the strong coupling limit (f ¼ 1). The inversion splitting of spin–orbit vibronic levels rationalizing the reduction of the orbital magnetic moments is schematically presented.

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article

Chemical Science

Fig. 11 Calculated values of cT (H ¼ 1000 Oe) at 1.8 and 300 K as a function of the vibronic coupling parameter f.

E E dxy ; MS ¼ 2; c0 Q0 þ Q0 dx2 y2 ; MS ¼ 2; c0 Q0 Q0 o o 2 3 d1 izg0;0 þ d2 4 5 izg0;0 þ d2 d1 (17) 0

0

0

0

|dx2y2 ,MS ¼ 2,c0(Q Qo)i and ¼ 2,c0(Q + Qo)i (see Fig. 10). Being of the same energy (d1 ¼ 0), these two wavefunctions are now mixed to rst order by spin–orbit coupling through the matrix element izg0,0 (d2 ¼ 0), with g0,0 given by exp(Qo2) (eqn (17)). The latter describes the vibrational overlap 0 0 0 0 between two displaced c0(Q Qo) and c0(Q + Qo) ground state harmonic oscillator wavefunctions. Thus, the energy gap 2z, being of the order of 600–800 cm1 in a static limit, now becomes strongly reduced by the quantity g0,0 (the Ham reduction factor), which exponentially decreases with 0 increasing shis 2Qo. As illustrated by the dependence of cT on f (see Fig. 11, as well as the ESI† for a similar but less monotonic eﬀect on the magnetization), for intermediate Renner–Teller couplings, pﬃﬃﬃ which imply ð1=2 2Þfgz2ðz þ h- uÞ, Fig. 2, right), a discontinuous change of the vibronic wavefunction and reduction of the orbital momenta takes place. Under these conditions, the nominal ground rML ¼ 2,MS ¼ 2, c0(Q0 )i and excited rML ¼ 2,MS ¼ 2, c2(Q)i wavefunctions start to mix strongly, thus leading to large reductions of the orbital moments. Nuclear probability distributions also imply superposition between ground state harmonic wavefunctions (c0(Q0 )) with higher excited vibrational states (in the given illustration with the second harmonic c2(Q0 ), Fig. 2). This induces large amplitude motions and dynamic distortions. Such a behavior may not apply to the situation in the solid state where, due to crystal packing forces (d1, d2 in eq. 17 s 0), transitions from dynamically averaged distorted congurations to statically distorted structures can take place. This point of view is supported by the observation that the FeC2 core in complex 2 was reported to be linear, while a derivative with a bent FeC2 geometry in Fe(Ar)2 (C–Fe–C ¼ 159.34(6) ) has also been reported.57 Likewise, while a distorted X-ray structure of 6 was reported, the EPR spectrum of the same compound in solution is only compatible with a more linear complex.30 It is remarkable that by using this dynamic Renner–Teller coupling model, room temperature 1

|d1xy,MS

This journal is ª The Royal Society of Chemistry 2013

values of cT for complexes 2–5 could be tted with a single adjustable parameter f that is conned to the narrow range between f ¼ 0.142 0.015 (see Table 4). At lower temperatures, however, smaller values of f (0.082–0.099) were required to t the susceptibility. One would expect the inuence of vibronic coupling to scale with temperature, and therefore f should increase with increasing T. Likewise, at lower temperatures, one would expect the value of f to decrease in concert with the increasing inuence of the spin–orbit coupling, which attempts to mitigate the vibronic eﬀects in order to sustain the orbital angular momentum, a so-called inverse Jahn–Teller eﬀect.58–60 The proposed underlying nuclear dynamics of these linear X– Fe–X complexes would be expected to show up in the ellipsoids of thermal motion.76–79 An inspection of the low-temperature (T ¼ 90(2) K for 1 and 3–7 and 100(2) K for 2) structures of complexes 1–6 indeed lends support the notion of vibronic activity in the rst coordination sphere of the FeII centers. Temperature- and eld-dependent structural studies should give more detailed information about this interesting phenomenon. 3.2.3 NUCLEAR DYNAMICS, LOW SYMMETRY LIGAND FIELDS, AND MAGNETIC RELAXATION. A large reduction of the magnetic susceptibility and magnetization beyond the values predicted by the static model is also observed for complex 6 with a bent structure. Interestingly, it too shows anomalous thermal ellipsoids, similar to those encountered for 1–5.55 Following the concept of Section 3.2.2, we have to assume that some residual vibronic activity remains in the distorted FeN2 core of 6. Two critical remarks should be made regarding the quantitative aspects of the Renner–Teller model presented in Sections 2.3 and 3.2.2. First, as has been stated in Section 3.1, the actual symmetry of all complexes 1–7 is not DNh but lower, generally C1, and the electronic ground state, assumed to be electronically doubly degenerate (5E) is actually split. Thus, any vibronic activity of the kind discussed in Section 3.2.2 should be viewed as being of the pseudo Jahn–Teller type. Second, the actual molecular complexes are large and possess a huge number of degrees of freedom. Thus, many vibrations of 3-type may be involved in vibronic coupling, which leads to an unapproachable multimode dynamic pseudo Jahn–Teller coupling problem.

Fig. 12 Experimental cT data (H ¼ 1000 Oe) for complex 6 (red squares) and theoretical values calculated using a model80,81 accounting for the simultaneous presence of the low-symmetry ligand ﬁeld (strain) and vibronic coupling of variable strength f (where f ¼ 0 corresponds to the static limit of no vibronic coupling).

Chem. Sci., 2013, 4, 139–156 | 149

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

Employing complex 6 as a model and following the general theory of Ham,80,81 the eﬀect of the static distortion on the magnetic properties can be accounted for by considering vibronic coupling and lower symmetry ligand elds (strain) as independent perturbations. The latter is quantied by the strain energy matrix Hstrain deduced here directly from the mapping of the NEVPT2 results for the quintet state manifold onto ligand eld theory (see ESI†). The dependence of the magnetic susceptibility on the vibronic coupling strength under the strain inuence for complex 6 is depicted in Fig. 12. It follows from these results that the combined action of lowered symmetry and vibronic coupling have a crucial eﬀect in reducing the magnetic susceptibility from its static limit (with a calculated room temperature value of cT z 3.95 cm3K mol1 for f ¼ 0) to values closer (cT ¼ 3.05 cm3K mol1 for f ¼ 1) to the experimentally reported value of cT ¼ 2.87 cm3K mol1.55 The observed (and calculated) Curie–Weiss behavior of 6 results from the even population of the lowest lying vibronic energy levels (at 0.0, 0.051, 2.32, 3.05, and 3.61 cm1), which are well-separated from other excited vibronic spin states. The combination of reduced symmetry and vibronic coupling also has a crucial eﬀect on the magnetic relaxation time, s. Low-temperature (T ¼ 2 K) eld-dependent magnetic relaxation data have been used to quantify contributions to s from quantum tunneling (st) and direct relaxation (sd) mechanisms according to eqn (18) (ref. 55) (see Table 3 for a list of B1, B2, and AH2 deduced from a least square t to such data). Expressions connecting B1, B2, and A with tunnel-splitting of the ground state magnetic pair DE, the eﬀective g-tensor value along the easy direction (gz), and the 1 s1 ¼ s1 t þ sd ¼

B1 þ AH 2 T 1 þ B2 H 2

(18)

B1 ¼ DE2s1/2

(19)

B2 ¼ (bgzs1/2)2 2 3k Vs-ph gz b A¼ 2ph4 rvS 5

(20) (21)

Table 5 Intrinsic life-times (s1/2), tunnel-splitting energies (DE), and spin– phonon coupling parameters (Vs–ph) obtained from B1, B2, and A values deduced from the ﬁeld-dependent magnetic relaxation data for complexes 1–5 at 2 K

s1/2 (s) 1a 2b 3c 4d 5e

1.48 2.27 4.93 4.27 7.43

1010 1011 106 1011 107

DE (cm1)

Vs–ph (cm1)

so (s)1

Ueﬀ(cm1)1

6.93 107 5.10 107 0.002 2.85 106 0.003

0.017 0.024 0.045 0.078 0.133

1 1011 4 109 5 109 4 108 3 107

181 146 109 104 43

a gz ¼ 11.66, computed from CASSCF + NEVPT2 using the X-ray geometry and r ¼ 1.149 g cm3. b gz ¼ 11.95, computed from CASSCF + NEVPT2 using the X-ray geometry and r ¼ 1.118 g cm3. c gz ¼ 9.60, calculated with a dynamic vibronic coupling model using f ¼ 0.15 and r ¼ 1.182 g cm3. d gz ¼ 9.60, calculated with a dynamic vibronic coupling model using f ¼ 0.15 and r ¼ 1.127 g cm3. e gz ¼ 9.60, calculated with a dynamic vibronic coupling model using f ¼ 0.15 and r ¼ 1.203 g cm3.

150 | Chem. Sci., 2013, 4, 139–156

Fig. 13 Variation of the spin–phonon coupling parameter Vs–ph across the series from 1 to 5.

dipole–dipole spin–phonon coupling parameter, Vs–ph,82 respectively, are given in eqn (19)–(21). In addition, the intrinsic life time of the magnetic ground state level s1/2 (for B1 and B2), the sound velocity (vS), and the mass density r (for A) have been taken into account. Adopting a realistic value of 1.20 km s1 for vS,83 the mass density r from X-ray structures and the ab initio values of gz (static, 1–2, or vibronic, 3–5), s1/2, DE and Vs–ph were deduced (see Table 5) using the reported values B1, B2, and A (Table 3).55 There is no clear trend for the changes of s1/2 across the series 1– 6, which also diﬀer from the lifetimes so due to the thermally activated Orbach relaxation mechanism. Impressively, there is clear trend of the spin–phonon coupling parameter Vs–ph, which increases from 1 to 5 (see Fig. 13). With one exception, complex 4, the tunnel-splitting energy DE follows the same trend. It increases dramatically ongoing from 1 and 2 to complexes 3 and 5. Not unexpectedly, no relaxation time data could be recorded for complex 6. The low-symmetry ligand eld in this complex leads to a 1 : 1 mixing (via the matrix element of 475 cm1) between the |ML ¼ +2> and |ML ¼ 2> electronic levels, in addition to a mixing of |ML ¼ 0> in the |ML ¼ 2> pair due to mixing via the oﬀ-diagonal matrix element of 1602 cm1. Both eﬀects reduce the orbital moments and facilitate quantum tunneling of the magnetization. Similar eﬀects on the relaxation times for complexes 1–5 emerge from the plots of the corresponding matrix elements (see ESI†). A second eﬀect on the relaxation time at elevated temperature is due to the narrowing of the energy gap between the ground and the excited magnetic sublevels (see experimentally deduced values of Ueﬀ included in Table 5 in comparison with the energy gap between the energy levels marked with red circles in Fig. 8, lower). The anisotropy-reducing eﬀect of the low symmetry decreases on further symmetry lowering from nearly C2v (in 1, 3, and 4 with one lone pair) to C1 (in 5 with two lone pairs) and can be ascribed to bonding eﬀects arising from the next-nearest neighboring atoms of the FeII centers (see Section 3.3). We note, however, that the changes of these matrix elements across 1–6 are not monotonic and do not follow the observed trend in s across the series.55 The reasons for such diﬀerences may be twofold: (i) thermal ellipsoids of the L–Fe–L moieties (see Fig. S1† in ref. 55) show that contributions from vibronic coupling may be present in all complexes, and (ii) secondary interactions of the FeII center with next nearest neighboring C

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

Chemical Science

Table 6 Angular overlap parameters (in cm1) from an analysis of the multiplet energies calculated using NEVPT2 of FeX2 complexes 1–7 and the truncated linear model clusters FeL2 (L ¼ CH3, NH2, OH)

Parameter

1

2

3

4

5

6

7

Fe(CH3)2

Fe(NH2)2

Fe(OH)2

es eps epc s(AOM)a DE(5A1–5B1) E(5A1) s, pc E(5B1) ps

3351 5137 1828 349 442 660 248

2513 2364 2364 68 18 310 292

4418 3973 932 344 373 512 139

4512 3860 1018 464 346 497 151

5255 3397 2439 493 108 444 336

5291 3414 884 794 308 440 132

3977 4530 2321 189 291 607 316

1799 1757 1757 431 15 236 221

2478 5354 1454 223 519 717 198

3560 4478 2921 136 221 599 378

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

a

Standard deviations between calculated (using the listed set of AOM parameters) and NEVPT2 matrix elements within the quintet state manifold.

atoms might be important. This is particularly relevant in 3–6, where p-electron lobes due to C(sp2) atoms from the phenyl substituents make relatively short contacts providing s/p overlap to the FeII centers (Fe/C ¼ 2.588, 2.765, 2.792, and ˚ decreasing from 6 to 5 to 4 to 3, respectively). Such 2.817 A, interactions are absent in 1 and 2 where Fe–C(sp3) contacts ˚ in 1 and occur at much longer distances (2 3.621, 2 3.587 A ˚ 2 3.275, 2 3.369, and 2 3.504 A in 2). 3.3

Ligand eld analysis of the ab initio results

The AOM parameters es, epc, and eps derived from the CASSCF + NEVPT2 results are listed in Table 6. Compared to other studies,70 standard deviations between LF (calculated using the AOM parameter set) and ab initio matrix elements here are in the expected range and show the adequacy of the LF approach for the studied complexes. The AOM parameters are consistent with values resulting from the t of the spectrum of the linear complex FeCl2 (es ¼ 3500 cm1, ep ¼ 2300 cm1).84 The origin of the anomalously low calculated values of the parameter es (in particular for the FeC2 complex 2) originates from the stabilizing eﬀect of 4s–3d mixing, which reduces largely the Fe–X s-antibonding interactions in the nominally dz2 type MO (see Section 3.1). Because of this stabilizing eﬀect (and in contrast to the results obtained for the series of [Fe(tpaR)] complexes),22,23 a correlation between es and the Lewis ligand basicity is not observed (see ESI†). Thus, the lowest value of es in complex 2 (see Table 6) correlates with the greatest Lewis basicity for the C ligator. Table 6 also reports AOM parameters for the truncated model complexes Fe(CH3)2, Fe(NH2)2 and Fe(OH)2. From a comparison between the sets of parameters of the model complexes with those of 1–7, we can conclude that there is a signicant tuning of the ligand eld strength for each type of donor, C, N, and O, by the structure (substituents) of the extended ligand framework. As follows from the parameter ratio eps/epc [1, there is a large p-bonding anisotropy for the amido ligands in 1, 3, 4, 6, and 7, and the large values of eps characterize the amido ligands as strong p-donors. For N being involved in two strong bonds to neighbor atoms, there are no orbitals for p bonding in the Fe–NR2 plane. One should therefore expect epc to be zero. That this is not the case implies that there are large electrostatic contributions to the LF parameters for FeN2 complexes 1, 3, 4, 6, and 7. A similar conclusion can be

This journal is ª The Royal Society of Chemistry 2013

Fig. 14 Dependence of the quintet term energies on the distortion angle q (see Fig. 3) for linear complexes with FeC2 (C2v, top), FeN2 (C2v, middle), and FeO2 (C2h, lower) cores, as obtained using the set of parameters for complexes 2, 4, and 5, respectively (see Table 6).

made based on the non-zero eps ¼ epc ¼ ep parameters deduced from the ab initio results for complex 2 (compare with the zero overlap due to such kind of interaction emerging from Table 1).

Chem. Sci., 2013, 4, 139–156 | 151

View Article Online

Chemical Science

Edge Article

Table 7 Interelectronic repulsion (B and C) and spin–orbit coupling (z) parameters (in cm1) from an analysis of the multiplet energies calculated using NEVPT2 of FeX2 complexes (1–7)a

B C s(B, C) z s(z)

1

2

3

4

5

6

7

1512 3245 1012 413 44

1418 3564 402 407 2

970 3782 1003 426 66

822 3965 1072 459 114

1090 3734 952 420 60

602 4364 746 822 274

1833 3030 325 591 225

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

a

Standard deviations s between the energies of electronic multiplets, calculated using the given set of parameters B, C (deduced from a least squares t to energies of the ground state quintet to triplet excited states transitions) and z (from a least squares t to the spin– orbit split terms of the 5E ground state) and the NEVPT2 (B and C) and NEVPT2 + SOC (z) results.

It was pointed out in Section 3.1 that bonding anisotropy reduces the symmetry from approximately C3v (for 2 and Fe(CH3)2) to approximately C2v in the FeN2 cores of 1, 3, 4, 6, and 7. Values of the energy D(5A1–5B1) – the splitting between the upper and lower components of the 5E ground terms, were computed with AOM parameters (see Table 6) assuming an arbitrary but xed value of the angle q ¼ 15 . This energy correlates directly with the term g(Qx2 + Qy2) (see eqn (5)) and thus with the eﬀect of vibronic pseudo Jahn–Teller coupling on the magnetic anisotropy (Section 3.2). This can be seen in Fig. 14, which shows that the energies of 5A1 and 5B1 increase upon bending because the two states are being destabilized by s, pc, and ps antibonding interactions, respectively. Thus, the splitting D(5A1–5B1) appears as a combination of the eﬀects of s, pc, and ps antibonding interactions. Distortions also lead to a lowering of the orbital moments because of mixing of the 5A1(dz2 |2,0>) state into the 5A1 dx2y2 |2,2>+|2,2> state. In addition, s–d mixing further lowers 5A1(dz2) and contributes to the reduction of the orbital angular momentum. Finally, at acute values of the angle q, an avoided crossing leads to a switch from a 5A1(dx2y2) to a 5A1(dz2) electronic ground state. This switch quenches the orbital angular momentum (Table 7). The parameterization given by the AOM with diagonal energy terms described by s (for M(dz2)–X(pz)), in-plane (pc for M(dxz)– X(px)), and out-of-plane (ps for M(dyz)–X(py)) antibonding interactions between M and X, is only justied in complexes with strictly linear (epc ¼ eps ¼ ep) or two-fold (C2v) symmetry for each Fe–X fragment. This situation can change in complexes with composite ligands, where, say, carbon atoms attached to a given sp2-type N donor atom can aﬀect its lone pair from being optimally aligned for s-bonding with the metal. The physical implications of such bent bonds (or “misdirected valence”) have been discussed by Liehr in relation to the optical rotatory power in tri- and digonal dihedral compounds.85,86 As judged by the standard deviations in Table 6, the overall success of the standard LF model (where misdirected valence is neglected) with AOM parameters es, eps, and epc is quite high. Yet, as expected for complexes 5, 4, and the bent complex 6, all possessing Cs or even lower (C1) Fe–X pseudosymmetries, standard deviations (493, 464, and 794 cm1, respectively) are larger than for the

152 | Chem. Sci., 2013, 4, 139–156

complexes with the more regular structures: FeC2 (C3v, s ¼ 68 cm1) and, to a lesser extent, the FeN2 complexes 1, 3, and 7 (C2v, s ¼ 349, 344, and 189 cm1, respectively). The extra lone pair located in the Fe–O–R plane of the FeO2 complex 5 (see Fig. 4) has the proper symmetry for both s and pc overlap. Keeping to the linear O–Fe–O geometry, this is expected to create an oﬀ-diagonal matrix element hdz2rVlone_pairrdxzi ¼ 2espc and to aﬀect the nominal values of es and epc. As has been pointed out by Gerloch et al.,87,88 in the general case of a Fe–X bond with pseudosymmetry C1, up to six AOM parameters for a given ligand have to be introduced (extended AOM, diagonal es, eps, epc and oﬀ-diagonal espc, espc, epcs). While there is little hope in obtaining much insight from such an over-parameterized model (the data base from optical spectroscopy is too limited in order to unambiguously extract the model parameters; see ref. 87 and 88 for attempts to do this), it is worthwhile to reconsider the more complete ab initio results in the light of this concept. Numerical data (see ESI†) given by the 1 : 1 mapping of the ab initio NEVPT2 data onto LFT for complex 5 leads to the following conclusions: (i) There is full support from ab initio theory for the expected s–p mixing between the rddz2i and rddxzi orbitals. The energetic eﬀect of the C2v to the Cs symmetry lowering is calculated not to be very large (espc ¼ 420 cm1) but comparable to that of the symmetry lowering from Cs to C1 (rddxzi–rddyzi, epcs ¼ 409 cm1). (ii) Bonding anisotropy implicated by a lowered actual symmetry causes 5E(dx2y2, dxy) in-state mixing (edpc ¼ 217 cm1) and rst-order splitting (edc eds ¼ 138 cm1), eﬀects that are ignored in conventional AOM modeling. Such mixings are counterintuitive and must be electrostatic in origin. (iii) The largest oﬀ-diagonal terms are calculated between 5 E(dx2y2, dxy) and 5A1(dz2) (esdc ¼ 1302 cm1, esds ¼ 828 cm1), but are ignored in the extended AOM. These terms lead to a mixing of 5A1 into 5E(dx2y2, dxy) and thus reduce the orbital momenta (see above). However, the 5A1(dz2)–5E(dx2y2, dxy) energy separation is relatively large (10 483 cm1), which somewhat lessens this eﬀect. While not being favorable for the single-molecule magnet behavior of the considered complexes, spatial asymmetries leading to matrix elements of the type hdz2rVlone_pairrdxzi ¼ 2espc are responsible for chirality leading to natural circular dichroism (NCD) in chelate complexes with highly-symmetric MXn (n ¼ 2–6) cores. The combination of this property with that of a high-spin FeII center, providing coexistence of spatial asymmetry (chirality leading to a parity break) and magnetization (causing a break of time reversal symmetry) can lead to optically active magnets (or magneto-chirality) and to magnetochiral dichroism with non-polarized light.89 As magnetic chiral media are intrinsically magnetoelectric, electrical reading/ writing in the magnetic state is possible, a feature that is currently being pursued in the rising eld of molecular multiferroic materials. With a bistable ground magnetic state E and A1 and A2 excited states, as found in complexes 1–7, a combination with chirality in properly selected enantiopure derivatives seems a very promising direction for further exploration.

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

4

Conclusions

(1) CASSCF/NEVPT2 calculations of the electronic multiplets of two-coordinate FeII complexes with C, N, and O donor ligands have been used to analyze the bonding within complexes 1–7 and to trace the eﬀects of the next-nearest atoms to the metal center on the Fe-ligand bonds. Angular overlap model parameters deduced from ab initio data, along with DFT calculations performed on linear Fe(CH3)2, Fe(NH2)2, and Fe(OH)2 model complexes, demonstrate that the respective properties are strongly aﬀected by the supporting ligand scaﬀold (N(CSi) in 1, C(Si)3 in 2, N(HC) in 3, 4, and 6, O(C) in 5, and N(C)2 in 7). Due to these bonds, the approximate local Fe–X pseudosymmetry is lowered from C3v for Fe–C(sp2) to C2v for Fe–N(sp2) to Cs for Fe– O(sp), leaving one, two and three ligand lone pairs for bonding to FeII, respectively. The bonding anisotropy, increasing in this sequence, causes a splitting of the doubly degenerate ground and excited state levels assumed respectively as 5D(dx2y2, dxy) and 5P(dxz, dyz) for linear FeX2 complexes. (2) Spin orbit coupling, here accounted for by quasidegenerate perturbation theory (QDPT) in the basis of the non-relativistic CASSCF wavefunctions and diagonal NEVPT2 corrections to the CASSCF energies, leads to magnetic sublevels of 5E parentage. Low symmetry splitting of the doubly degenerate E ground state magnetic sublevel pair, caused by the bonding anisotropy, is strongly suppressed by SOC, but shows up to the full extent in the second doubly degenerate excited magnetic sublevel pair. Using static geometries taken from the crystal structures, low-temperature (T ¼ 1.8–5 K) isothermal magnetization data and magnetic susceptibilities (for 1 and 2) could be reasonably well reproduced. (3) A dynamic 5E53 vibronic coupling model of the Renner– Teller type has been employed to explain why the experimentally determined magnetization and susceptibility data for complexes 3–6 are systematically lower than the theoretically predicted results, assuming only static geometric distortions. The model incorporates three model parameters (g, j, and h- u3, corresponding to the Renner–Teller vibronic coupling constant, anharmonicity, and harmonic energy parameters, respectively) that were adjusted to the adiabatic ground state potential of a distorted Fe(CH3)2 model complex. Vibronic reductions of orbital contributions to the net magnetic moment exceed by far the orbital moment quenching induced by covalency. Following this model, it was possible to t the low (T ¼ 2 K) and room (T ¼ 300 K) temperature magnetic susceptibility data for complexes 2–6 in terms of a single parameter f, the vibronic coupling strength, which can vary between 0 (no vibronic coupling) and 1 (strong vibronic coupling). The best t values for f fall into a narrow range at 0.142 0.015. The given range of f nearly coincides with borderline of a discontinuous change from weak (f < 0.1) to strongly (f > 0.1) coupled electronic and nuclear motions, where vibronic coupling is being quenched by SOC (f < 0.1) or vice versa (f > 0.1). It is conceivable that in a solid, large amplitude movements will readily drive the system from a dynamically averaged into a static distorted nuclear conguration. The very diﬀerent magnetic behaviors reported for complexes 1–2 and 3–6 are a clear manifestation of such

This journal is ª The Royal Society of Chemistry 2013

Chemical Science behavior, and should be the subject of more detailed structural, magnetic, and spectroscopic studies. (4) A general method allowing a 1 : 1 mapping of the ligand eld matrix, as deduced from ab initio CASSCF + NEVPT2 calculations, onto corresponding AOM energy expressions was used to obtain values of the antibonding energies of s (es), the in- (epc) and out-of- (eps) plane p-type. The parameters show: (i) a large reduction of es due to 3dz2–4s mixing (hybridization) typical for linear X–M–X transition metal complexes, (ii) pbonding anisotropy reected in eps > epc for the Fe–N(sp2) and Fe–O(sp) type complexes, and (iii) framework hyperconjugative eﬀects manifested in values of ep assumed otherwise to be zero (ep for C(sp3) and epc for N(sp2)). In the same context, ligand eld matrix elements neglected in common AOM parameterization schemes, but accounted for by its extended versions (such as s–p mixings and misdirected valence) could be traced back and veried. Other couplings (dx2y2–dz2, dxy–dz2, and dxy– dx2y2), which, due to the high level of over-parameterization have not been discussed before, emerged from our analysis. (5) Based on the theoretical analysis, the following guidelines for generating new single-molecule magnets with improved magnetic anisotropies and relaxation times can be formulated: (i) enhancement of the spin–orbit coupling and concomitant suppression of the vibronic coupling is predicted to improve the anisotropy barrier Ueﬀ (see Fig. 8). Both features can be met by replacing the C, N, or O donor atoms with their heavier analogues, such as Si, P, or S. Indeed, some FeS2 moieties have already been reported.90 Ligand spin–orbit coupling, increasing in this direction may add to the metal one, thus compensating for the enhanced metal–ligand covalence, which tends to act in the opposite direction (relativistic nephelauxetic eﬀect). Such an increase in molecular magnetic anisotropy as a result of the coordination of increasingly heavier ligand atoms has been demonstrated recently in octahedral complexes of CrIII.91 Additionally, vibronic coupling, which decreases with increasing metal–ligand covalency, is expected to support a larger Ueﬀ. A nice manifestation of such an eﬀect is a recently reported CoS4 single-molecule magnet, the rst example of a transition metal complex exhibiting slow magnetic relaxation under zero applied dc magnetic eld.92 (ii) Metal–ligand bonds with C3v and C2v local pseudosymmetries, enforced by the next-nearest metal neighbors (C(sp3) and N(sp2)), are preferable to lower symmetry ones (O(sp2)), which create large matrix elements between the ground state MJ sublevels. (iii) Avoiding secondary metal–ligand interactions through the use of sterically encumbering ligands with aliphatic (1, 2) rather than aromatic substituents (3–5) has a favorable eﬀect on the relaxation time. Along the same line, bulky ligands of the former type tend to support linear FeX2 cores and thus oppose in an indirect way unfavorable vibronic coupling. (iv) Suppression of dipolar spin–spin interactions between magnetic centers in the solid will increase the relaxation time for the direct process. It is this kind of interaction which shows the expected trend of relaxation times (see Fig. 13) across the series. Thus decoupling of the molecule from the lattice is an

Chem. Sci., 2013, 4, 139–156 | 153

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science important goal. Aside from the usual approaches used to achieve this (e.g., dilution of the single-molecule magnets by substitution in a diamagnetic isomorphic compound or in frozen solution), stabilization of the molecules on a metal (usually gold) surface provides a modern way of approaching this. One possibility of doing this is given by using appropriately chosen spacer molecules that can “wire” a single-molecule magnet to a gold surface.1 Another method, involving vapor deposition, should be facile for certain mononuclear transition metal complexes that are neutral and can sublime. For example, complex 2 is easily sublimable.93 In the context of the FeX2 single-molecule magnets, a possible target would be an – AuS3C–C^C–Fe–C^C–CS3Au – structure. Unfavorable vibronic coupling which tends to stabilize bent structures will be suppressed within the constraints given above. (6) The large magnetic anisotropy due to unquenched rst order orbital momentum in the 5E ground states of the considered FeX2 complexes leads to large anisotropy barriers. However, quantum tunneling of the magnetization is particularly eﬃcient owing to the small value of S ¼ 2 and the lowsymmetry perturbations of the kind discussed in Sections 3.2.3 and 3.3. Thus, the search for better single-molecule magnets that stay magnetized at elevated temperatures requires a combination of a large Ueﬀ and a small quantum tunneling rate. This goal is only partly (due to intrinsic transversal magnetic elds stemming from dipole–dipole interactions which cannot be avoided in a solid) achieved by choosing Kramers rather than non-Kramers Fe(II) (S ¼ 2) ions, as was shown in the recently reported [Co(SPh)4]2 (S ¼ 3/2) complex.92 The condition of larger Ueﬀ (large/small spin–orbit/vibronic coupling) and a small quantum tunneling of the magnetization (large total moments MJ) seems to be ideally met in complexes of rare earths such as phthalocyanine (pc) double decker complexes, e.g. (pc)2TbIII.94 A similar possibility for complexes of 3d metals employs low-coordinate Fe(II) (introducing large Ueﬀ) ferromagnetically coupled with several MnII (S ¼ 5/2, introducing a large spin). Such a synthetic strategy has yet to be explored.

Acknowledgements This research was supported by NSF grant CHE-1111900. We thank Tyco Electronics for fellowship support of J.M.Z.

Notes and references 1 M. Mannini, F. Pineider, P. Sainctavit, C. Danieli, E. Otero, C. Sciancalepore, A. M. Talarico, M.-A. Arrio, A. Cornia, D. Gatteschi and R. Sessoli, Nat. Mater., 2009, 8, 194. 2 M. N. Leuenberger and D. Loss, Nature, 2001, 410, 789. 3 A. Ardavan, O. Rival, J. J. L. Morton, S. J. Blundell, A. M. Tyryshkin, G. A. Timco and R. E. P. Winpenny, Phys. Rev. Lett., 2007, 98, 057201. 4 P. C. E. Stamp and A. Gaita-Ari~ no, J. Mater. Chem., 2009, 19, 1718. 5 F. Torres, J. M. Hern´ andez, X. Bohigas and J. Tejada, Appl. Phys. Lett., 2000, 77, 3248.

154 | Chem. Sci., 2013, 4, 139–156

Edge Article 6 R. Sessoli, D. Gatteschi, A. Caneschi and M. A. Novak, Nature, 1993, 365, 141. 7 D. Gatteschi, R. Sessoli and J. Villain, Molecular Nanomagnets, Oxford University Press, New York, 2006 and references therein. 8 N. E. Chakov, S.-C. Lee, A. G. Harter, P. L. Kuhns, A. P. Reyes, S. O. Hill, N. S. Dalal, W. Wernsdorfer, K. Abboud and G. Christou, J. Am. Chem. Soc., 2006, 128, 6975. 9 C. J. Milios, A. Vinslava, W. Wernsdorfer, S. Moggach, S. Parsons, S. P. Perlepes, G. Christou and E. K. Brechin, J. Am. Chem. Soc., 2007, 129, 2754. 10 C. Sangregorio, T. Ohm, C. Paulsen, R. Sessoli and D. Gatteschi, Phys. Rev. Lett., 1997, 78, 4645. 11 S. M. J. Aubin, N. R. Dilley, L. Pardi, J. Krzystek, M. W. Wemple, L.-C. Brunel, M. B. Maple, G. Christou and D. N. Hendrickson, J. Am. Chem. Soc., 1998, 120, 4991. 12 A.-L. Barra, A. Canneschi, A. Cornia, F. Fabrizi de Biani, D. Gatteschi, C. Sangregorio, R. Sessoli and L. Sorace, J. Am. Chem. Soc., 1999, 121, 5302. 13 S. Accorsi, A. L. Barra, A. Caneschi, G. Chastanet, A. Cornia, A. C. Fabretti, D. Gatteschi, C. Mortal` o, E. Olvieri, F. Parenti, R. Sessoli, L. Sorace, W. Wernsdorfer and L. Zobbi, J. Am. Chem. Soc., 2006, 128, 4742. 14 L. Gregoli, C. Danieli, A.-L. Barra, P. Neugebauer, G. Pellegrino, G. Poneti, R. Sessoli and A. Cornia, Chem.– Eur. J., 2009, 15, 6456. 15 F. Neese and D. A. Pantazis, Faraday Discuss., 2011, 148, 229. 16 O. Waldmann, Inorg. Chem., 2007, 46, 10035. 17 F. Neese and E. I. Solomon, Inorg. Chem., 1998, 37, 6568. 18 C. J. Milios, C. P. Raptopoulou, A. Terzis, F. Lloret, R. Vincente, S. P. Perlepes and A. Escuer, Angew. Chem., Int. Ed., 2004, 43, 210. 19 E. K. Brechin, C. Boskovic, W. Wernsdorfer, J. Yoo, A. Yamaguchi, E. C. Sa~ nudo, T. R. Concolino, A. L. Rheingold, H. Ishimoto, D. N. Hendrickson and G. Christou, J. Am. Chem. Soc., 2002, 124, 9710. 20 J. Villain, F. Hartman-Boutron, R. Sessoli and A. Rettori, Europhys. Lett., 1994, 27, 159. 21 W. H. Harman and C. J. Chang, J. Am. Chem. Soc., 2007, 129, 15128. 22 D. E. Freedman, W. H. Harman, T. D. Harris, G. J. Long, C. J. Chang and J. R. Long, J. Am. Chem. Soc., 2010, 132, 1224. 23 W. H. Harman, T. D. Harris, D. E. Freedman, H. Fong, A. Chang, J. D. Rinehart, A. Ozarowski, M. T. Sougrati, F. Grandjean, G. J. Long, J. R. Long and C. J. Chang, J. Am. Chem. Soc., 2010, 132, 18115. 24 Throughout this work electron congurations due to the high-spin Fe(II) d6 subshell will be denoted by orbitals which carry the extra electron in addition to the half-lled d5 shell. 0 25 A diﬀerent denition of MJ ¼ MS + ML/2, used to directly relate the magnetic moment with the free electron go ¼ 2 0 value (M ¼ mBgoMJH), was employed in ref. 46. Here, we return to the usual denition of MJ ¼ MS + ML which also correctly reects the transformation symmetry of the

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

26 27 28

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

29

30

31 32 33 34

35 36 37 38 39

40 41 42 43 44 45 46 47 48

wavefunction. Another denition treating the total moment in a S ¼ 1/2 pseudospin approach (used by the ESR community) denes the magnetic moment as M ¼ 0 mBmgeﬀH (geﬀ ¼ goSMJ, m ¼ 1/2). B. R. McGarvey and J. Telser, Inorg. Chem., 2012, 51, 6000. D. Dai and M.-H. Whangbo, Inorg. Chem., 2005, 44, 4407. W. M. Reiﬀ, A. M. LaPointe and E. H. Witten, J. Am. Chem. Soc., 2004, 126, 10206. W. M. Reiﬀ, C. E. Schulz, M.-H. Whangbo, J. I. Seo, Y. S. Lee, G. R. Potratz, C. W. Spicer and G. S. Girolami, J. Am. Chem. Soc., 2009, 131, 404. W. A. Merrill, T. A. Stich, M. Brynda, G. J. Yeagle, J. C. Fettinger, R. De Hont, W. M. Reiﬀ, C. E. Schulz, R. D. Britt and P. P. Power, J. Am. Chem. Soc., 2009, 131, 12693. M. Atanasov, P. Comba and C. A. Daul, Inorg. Chem., 2008, 47, 2449. M. Atanasov, C. A. Daul and C. Rauzy, Struct. Bonding, 2004, 106, 97. M. Atanasov, C. A. Daul and C. Rauzy, Chem. Phys. Lett., 2003, 367, 737. M. Atanasov and P. Comba, in The Jahn-Teller Eﬀect: Fundamentals and Implications for Physics and Chemistry, ed. H. K¨ oppel, H. Barentzen and D. R. Yarkony, Springer Series in Chemical Physics, Berlin, 2009, p. 97. ˚ Malmqvist and B. O. Roos, Chem. Phys. Lett., 1989, 155, P.-A. 189. K. Wolinski and P. Pulay, J. Chem. Phys., 1989, 90, 3647. ˚ Malmqvist, B. O. Roos, A. J. Sadlej and K. Andersson, P.-A. K. Wolinski, J. Phys. Chem., 1990, 94, 5483. ˚ Malmqvist and B. O. Roos, J. Chem. Phys., K. Andersson, P.-A. 1992, 96, 1218. ˚ Malmqvist, P. L. SerranoB. O. Roos, M. P. F¨ ulscher, P.-A. Andr´ es, and M. Merch´ an, Theoretical Studies of the Electronic Spectra of Organic Molecules, in Quantum Mechanical Electronic Structure Calculations with Chemical Accuracy, ed. S. R. Langhoﬀ, Kluwer, Dordrecht, 1994. ˚ Malmqvist, Phys. Chem. Chem. Phys., B. O. Roos and P.-A. 2004, 6, 2919. C. Angeli, R. Cimiraglia and J.-P. Malrieu, Chem. Phys. Lett., 2001, 350, 297. C. Angeli, R. Cimiraglia, S. Evangelisti, T. Leininger and J.-P. Malrieu, J. Chem. Phys., 2001, 114, 10252. C. Angeli, R. Cimiraglia and J.-P. Malrieu, J. Chem. Phys., 2002, 117, 9138. C. Angeli, B. Bories, A. Cavallini and R. Cimiraglia, J. Chem. Phys., 2006, 124, 054108. R. Maurice, C. de Graaf and N. Guih´ ery, J. Chem. Phys., 2010, 133, 084307. M. Atanasov, D. Ganyushin, D. A. Pantazis, K. Sivalingam and F. Neese, Inorg. Chem., 2011, 50, 7640. D. Maganas, S. Sottini, P. Kyritsis, E. J. J. Groenen and F. Neese, Inorg. Chem., 2011, 50, 8741. R. Maurice, R. Bastardis, C. de Graaf, N. Suaud, T. Mallah and N. Guih´ ery, J. Chem. Theory Comput., 2009, 5, 2977.

This journal is ª The Royal Society of Chemistry 2013

Chemical Science 49 R. Maurice, N. Guih´ ery and C. de Graaf, J. Chem. Theory Comput., 2010, 6, 55. 50 R. Maurice, A. M. Pradipto, N. Guih´ ery, R. Broer and C. de Graaf, J. Chem. Theory Comput., 2010, 6, 3092. 51 S. Vancoillie, J. Chalupsk´y, U. Ryde, E. I. Solomon, K. Pierloot, F. Neese and L. Rulȋˇsek, J. Phys. Chem. B, 2010, 114, 7692. 52 M. Atanasov and P. Comba, in Structure and Function, ed. P. Comba, Springer, 2010, pp. 74–79. 53 F. Neese, WIREs Comput. Mol. Sci., 2012, 2, 73. 54 ORCA, An ab initio, DFT and Semiempirical SCF-MO Package – Version 2.8, 20 September 2010by F. Neese, F. Wennmohs, with contributions from U. Becker, D. Bykov, D. Ganyushin, A. Hansen, R. Izsak, D. G. Liakos, C. Kollmar, S. Kossmann, D. A. Pantazis, T. Petrenko, C. Reimann, C. Riplinger, M. Roemelt, B. Sandh¨ ofer, I. Schapiro, K. Sivalingam, E. Valeev and B. Wezisla, Max-Planck Institut f¨ ur Chemische Energiekonversion, http://www.mpibac.mpg.de/bac/index_ en.php. 55 J. M. Zadrozny, M. Atanasov, A. M. Bryan, C.-Y. Lin, B. D. Rekken, P. P. Power, F. Neese and J. R. Long, Chem. Sci., 2012, DOI: 10.1039/c2sc20801f. 56 T. Vieaus, W. Schwarz, K. H¨ ubler, K. Locke and J. Weidlein, Z. Anorg. Allg. Chem., 2001, 627, 715. 57 C. Ni and P. P. Power, Chem. Commun., 2009, 5543. 58 R. S. Fishman and F. A. Reboredo, Phys. Rev. Lett., 2007, 99, 217203-1. 59 R. S. Fishman, S. Okamoto and F. A. Reboredo, Phys. Rev. Lett., 2008, 101, 116402-1. 60 R. S. Fishman and F. A. Reboredo, Phys. Rev. B: Condens. Matter Mater. Phys., 2008, 77, 144421. 61 P. Reis, R. S. Fishman, F. A. Reboredo and J. Moreno, Phys. Rev. B, 2008, 77, 174433. 62 F. Neese and E. I. Solomon, in Magnetism: Molecules to Materials, ed. J. S. Miller and M. Drillon, Wiley-VCH, Weinheim, 2003, vol. IV, pp. 345–466. 63 I. B. Bersuker, The Jahn–Teller Eﬀect and Vibronic Interactions in Modern Chemistry, Plenum Press, New York and London, 1984. 64 I. B. Bersuker, The Jahn–Teller Eﬀect, University Press, Cambridge, 2006. 65 E. Renner, Z. Phys., 1934, 92, 172. 66 G. Herzberg and E. Teller, Z. Phys. Chem., Abt. B, 1933, 21, 410. 67 J. A. Pople and H. C. Longuet-Higgins, Mol. Phys., 1958, 1, 372. 68 R. N. Dixon, Mol. Phys., 1965, 9, 357. 69 A. A. Petelin, Int. J. Quantum Chem., 1972, 6, 701. 70 M. Atanasov, D. Ganyushin, K. Sivalingam and F. Neese, Struct. Bonding, 2012, 143, 149. 71 C. K. Jørgensen, R. Pappalardo and H.-H. Schmidtke, J. Chem. Phys., 1963, 39, 1422. 72 C. E. Sch¨ aﬀer and C. K. Jørgensen, Mol. Phys., 1965, 9, 401. 73 B. N. Figgis and M. A. Hitchman, Ligand Field Theory and Its Applications, Wiley-VCH, NewYork, 2000. 74 H. Adamsky, with contributions from P. E. Hoggard, M. Atanasov and K. Eifert, AOMX, http://www.aomx.de.

Chem. Sci., 2013, 4, 139–156 | 155

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

75 D. Reinen, M. Atanasov and S.-L. Lee, Coord. Chem. Rev., 1998, 175, 91. 76 J. D. Dunitz and D. N. J. White, Acta Crystallogr., Sect. A: Cryst. Phys., Diﬀr., Theor. Gen. Crystallogr., 1973, A29, 93. 77 J. D. Dunitz, E. F. Maverick and K. N. Trueblood, Angew. Chem., 1988, 100, 910. 78 J. H. Ammeter, H. B. B¨ urgi, E. Gamp, V. Meyer-Sandrin and W. P. Jensen, Inorg. Chem., 1979, 18, 733. 79 M. Atanasov, W. K¨ onig, H. Craubner and D. Reinen, New. J. Chem., 1993, 17, 115. 80 F. S. Ham, in Electron Paramagnetic Resonance, ed. S. Geschwind, Plenum Press, New York, 1972, p. 1. 81 F. S. Ham, Phys. Rev., 1965, 138, 1727. 82 Vs–ph is related with the magnetogyric ratio for electrons, Nneigbors P 6 . 2 n – a ro;i g ¼ e/mc, the parameter a ¼ 2 i¼1

constant somewhat greater than unity, the magnetic pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ moment per ion m ¼ gJ Jð J þ 1Þ (in Bohr magnetons) and n –the number of magnetic ions per 1 volume as Vs–ph2 ¼ (3a/8)g2n2m2h- 2, A. Abragam and B. Bleaney, Electron Paramagnetic Resonance of Transition Ions, Clarendon Press, Oxford, 1970.

156 | Chem. Sci., 2013, 4, 139–156

83 V. Starovoitova, G. R. A. Wyllie, W. R. Scheidt, W. Sturhan, E. Ercan Alp and S. M. Durbin, J. Phys. Chem. B, 2008, 112, 12661. 84 C. W. DeKock and D. M. Gruen, J. Chem. Phys., 1966, 44, 4383. 85 A. D. Liehr, J. Phys. Chem., 1964, 68, 665. 86 A. D. Liehr, J. Phys. Chem., 1964, 68, 3629. 87 M. Gerloch, J. H. Harding and G. G. Woolley, Struct. Bonding, 1981, 46, 1. 88 A. J. Bridgeman and M. Gerloch, Prog. Inorg. Chem., 1997, 45, 179–281, p. 238, Table III. 89 C. Train, R. Gheorghe, V. Krstic, L.-M. Chamoreau, N. S. Ovanesyan, G. L. J. A. Rikken, M. Gruselle and M. Verdaguer, Nat. Mater., 2008, 7, 729. 90 T. Nguyen, A. Panda, M. M. Olmstead, A. F. Richards, M. Stender, M. Brynda and P. P. Power, J. Am. Chem. Soc., 2005, 127, 8545. 91 H. I. Karunadasa, K. D. Arquero, L. A. Berben and J. R. Long, Inorg. Chem., 2010, 49, 4738. 92 J. M. Zadrozny and J. R. Long, J. Am. Chem. Soc., 2011, 133, 20732. 93 A. M. LaPointe, Inorg. Chim. Acta, 2003, 345, 359. 94 N. Ishikawa, Struct. Bonding, 2010, 135, 211 and references therein.

This journal is ª The Royal Society of Chemistry 2013

EDGE ARTICLE

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Cite this: Chem. Sci., 2013, 4, 139

View Journal | View Issue

A theoretical analysis of chemical bonding, vibronic coupling, and magnetic anisotropy in linear iron(II) complexes with single-molecule magnet behavior† Mihail Atanasov,*ab Joseph M. Zadrozny,c Jeﬀrey R. Longc and Frank Neese*a The electronic structure and magnetic anisotropy of six complexes of high-spin FeII with linear FeX2 (X ¼ C, N, O) cores, Fe[N(SiMe3)(Dipp)]2 (1), Fe[C(SiMe3)3]2 (2), Fe[N(H)Ar0 ]2 (3), Fe[N(H)Ar*]2 (4), Fe[O(Ar0 )]2 (5), and Fe[N(t-Bu)2]2 (7) [Dipp ¼ C6H3-2,6-Pri2; Ar0 ¼ C6H3-2,6-(C6H3-2,6-Pri2)2; Ar* ¼ C6H3-2,6-(C6H2-2,4,6Pri2)2; Ar# ¼ C6H3-2,6-(C6H2-2,4,6-Me3)2], and one bent (FeN2) complex, Fe[N(H)Ar#]2 (6), have been studied theoretically using complete active space self-consistent ﬁeld (CASSCF) wavefunctions in conjunction with N-Electron Valence Perturbation Theory (NEVPT2) and quasidegenerate perturbation ¨ ssbauer theory (QDPT) for the treatment of magnetic ﬁeld and spin-dependent relativistic eﬀects. Mo studies on compound 2 indicate an internal magnetic ﬁeld of unprecedented magnitude (151.7 T) at the FeII nucleus. This has been interpreted as arising from ﬁrst order angular momentum of the 5D ground state of FeII center (J. Am. Chem. Soc. 2004, 126, 10206). Using geometries from X-ray structural data, ligand ﬁeld parameters for the Fe-ligand bonds were extracted using a 1 : 1 mapping of the angular overlap model onto multireference wavefunctions. The results demonstrate that the metal– ligand bonding in these complexes is characterized by: (i) strong 3dz2–4s mixing (in all complexes), (ii) pbonding anisotropy involving the strong p-donor amide ligands (in 1, 3–4, 6, and 7) and (iii) orbital mixings of the s–p type for Fe–O bonds (misdirected valence in 5). The interplay of all three eﬀects leads to an appreciable symmetry lowering and splitting of the 5D (3dxy, 3dx2y2) ground state. The strengths of the eﬀects increase in the order 1 < 5 < 7 6. However, the diﬀerential bonding eﬀects are largely overruled by ﬁrst-order spin–orbit coupling, which leads to a nearly non-reduced orbital contribution of L ¼ 1 to yield a net magnetic moment of about 6 mB. This unique spin–orbital driven magnetism is signiﬁcantly modulated by geometric distortion eﬀects: static distortions for the bent complex 6 and dynamic vibronic coupling eﬀects of the Renner–Teller type of increasing strength for the series 1–5. Ab initio calculations based on geometries from X-ray data for 1 and 2 reproduce the magnetic data exceptionally well. Magnetic sublevels and wavefunctions were calculated employing a dynamic Renner–Teller vibronic coupling model with vibronic coupling parameters adjusted from the ab initio results on a small Fe(CH3)2 truncated model complex. The model reproduces the observed reduction of the orbital moments and quantitatively reproduces the magnetic susceptibility data of 3–5 after introduction of the vibronic coupling strength (f) as a single adjustable parameter. Its value varies

Received 30th August 2012 Accepted 3rd October 2012

in a narrow range (f ¼ 0.142 0.015) across the series. The results indicate that the systems are near the borderline of the transition from a static to a dynamic Renner–Teller eﬀect. Renner–Teller vibronic activity is used to explain the large reduction of the spin-reversal barrier Ueﬀ along the series from 1 to

DOI: 10.1039/c2sc21394j

5. Based upon the theoretical analysis, guidelines for generating new single-molecule magnets with

www.rsc.org/chemicalscience

enhanced magnetic anisotropies and longer relaxation times are formulated.

a Max-Planck Institut fur Chemische Energiekonversion, Stifstr. 32–34, D-45470 Mulheim an der Ruhr, Germany. E-mail: [email protected]; frank. [email protected] b

Institute of General and Inorganic Chemistry, Bulgarian Academy of Sciences, Acad Georgi Bontchev Str. 11, 1113 Soa, Bulgaria

c

Department of Chemistry, University of California, Berkeley, CA, 94720, USA

† Electronic supplementary information (ESI) available: Full computational details, results, and formulae. Calculated molar dc susceptibility and magnetization data for 2–5 and NIR d–d absorption spectrum of 1. See DOI: 10.1039/c2sc21394j

This journal is ª The Royal Society of Chemistry 2013

1

Introduction

Considerable eﬀorts have been dedicated toward the synthesis and characterization of single-molecule magnets—paramagnetic molecules displaying magnetic bistability. The motivation for these studies lies in the interest in the potential future applications for such compounds in high-density information storage,1 quantum computing,2–4 and magnetic refrigeration.5 Single-molecule magnets are open shell spin systems,

Chem. Sci., 2013, 4, 139–156 | 139

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science which under an applied external direct current (dc) magnetic eld are magnetized and remain so upon removal of the eld. The phenomenon occurs at temperatures below a critical value, the blocking temperature TB. This property is intrinsically related to the existence of an energy barrier U ¼ S2|D| for the reversal of the magnetization (D is the axial zero-eld splitting parameter for the ground state of total spin S, frequently referred to as the magnetic anisotropy) by spin–phonon coupling and/or thermally assisted quantum tunneling, which usually renders the eﬀective barrier Ueﬀ smaller than U. The targeted large and negative quantity D implies orbital contributions to the spin from spin–orbit coupling in combination with an axial threefold or fourfold molecular symmetry (uniaxial anisotropy). Since the discovery of the eﬀect in the celebrated Mn12 single-molecule magnet (TB z 3.5 K, Ueﬀ up to 72 K),6–8 many such systems belonging to the same family or other ones – (e.g., Mn6,9 Fe8,10 Mn4,11 and Fe4 (ref. 12–14) have been found to exhibit a similar type of magnetic behavior. It was pointed out that, with the number of spin centers being the same, since rDr f 1/S2, a high value of S is not a necessary condition for large Ueﬀ values to occur.15 It is important to note that this mathematical relationship is not a feature that arises from cluster spin coupling,16 but instead follows from the fundamental theory of the zero-eld splitting interaction.17 This prediction is supported by experiment, as comparison between D values of Mnn complexes with diﬀerent nuclearity (n) and variable spinground states (S) shows: n ¼ 1, D ¼ 2.29 cm1, S ¼ 2,16 n ¼ 6, D ¼ 1.22 cm1, S ¼ 4 (ref. 18), n ¼ 12, D ¼ 0.5 cm1, S ¼ 10,6–8 n ¼ 6, D ¼ 0.43 cm1, S ¼ 12,9 and n ¼ 18, D ¼ 0.13 cm1, S ¼ 13.19 However, in favor of systems with a large total spin, one can quote that the relaxation time (s) for the thermally activated process is greatly enhanced by large values of S, as was pointed out on theoretical grounds (s f (S6/U3)exp(U/kBT)).20,7 It has been also shown (ref. 7, Chapter 6) that increasing total spin S leads to suppression of the quantum tunneling of the magnetization as quantied by the ground state (Landau–Zener) splitting DE(MS ¼ S) which vanishes exponentially with DE (MS ¼ S) f [Hx/(4rDrS)]2S, Hx – the intrinsic transversal magnetic eld. In MnIII- and FeIII-based single-molecule magnets, the magnetic anisotropy arises from favorable alignment of local Dtensors, which originate from mixing, via spin–orbit coupling, of the non-degenerate ground states of MnIII (d4, subject to static Jahn–Teller distortions) or of FeIII (d5) with excited electronic states bearing rst-order orbital angular momenta. The directed, favorable alignment of local anisotropy axes in a multinuclear transition metal complex is obviously a grand synthetic challenge that cannot be considered as being solved. Hence, another strategy to achieve more negative D-values is to focus on complexes with trigonal geometries and orbitally degenerate ground states 2S+1E. Hybrid ligand scaﬀolds of FeII with trianionic tris(pyrrolyl-a-methyl) amines (tpa),21 for example, enforce a three-fold coordination geometry around the FeII centers, which can result in unusually large values, such as D ¼ 40 cm1 for [K(DME)4][Fe(tpaMes)].22 The observation of slow relaxation of the magnetization in this complex with the presence of a small dc eld, with an eﬀective relaxation barrier 140 | Chem. Sci., 2013, 4, 139–156

Edge Article of Ueﬀ ¼ 42 cm1, provided the rst example of a mononuclear transition metal complex with single-molecule magnet-like behavior.22 Expanding on this discovery, a series of four structurally and magnetically well-documented compounds: [Fe(tpaR)] (R ¼ tert-butyl, mesityl, phenyl and 2,6-diuorophenyl) were reported to display similar properties tuned by a variation of the substituents R.23 In the trigonally elongated site imposed by the tpaR ligand, the (dxz,yz)1 electron conguration24 yields a contribution of ML ¼ 1 to the net spin moment of MS ¼ 2, resulting in a bistable MJ ¼ 3 (5/2 mB) ground state.25 The eﬀect of the orbital moment on the magnetic anisotropy would be enhanced in hypothetical trigonally compressed tetrahedral FeX4 (5E(dx2y2,xy)1)26 or linear FeX2 (5D(dx2y2,xy)1) complexes possessing a twice larger orbital contribution to the magnetic moment of ML ¼ 2.27 In one complex of the latter type, Fe [C(SiMe3)3]2 (2), very large orbital momentum contributions, equivalent to adding two full S ¼ 1/2 spins to the spin-only value of S ¼ 2, were demonstrated by an unusually large internal hyperne eld (Hint ¼ 151.6 T), as manifested in the M¨ ossbauer spectra and also by dc magnetization measurement.28 A similar but less pronounced hyperne eld (Hint ¼ 105 T) was later found in the compound Fe[N(t-Bu)2]2 (7), with the lower relative magnitude of Hint being attributed to the lower eﬀective symmetry imposed by the non-axially symmetric ligands.29 Additionally, experimental observation of quenched orbital angular momentum induced by a bent L–Fe–L angle was shown for the two-coordinate complex Fe[N(H)Ar#]2 (Ar# ¼ C6H3-2,6(C6H2-2,4,6-Me3)2) (6), in contrast to the linear Fe[N(H)Ar*]2 analogue (Ar* ¼ C6H3-2,6-(C6H2-2,4,6-Pri2)2) (4), which showed the large magnetic moment and internal hyperne eld suggestive of orbital angular momentum.30 Transition metal complexes with open d-shells have traditionally been treated by ligand eld theory (LFT). As a parametrical model, LFT can only be used for the sake of interpretation, rather than for the prediction of properties. Density functional theory (DFT), being broadly used in chemistry for the prediction of ground state geometries and properties of electronic states in molecules, is well suited for systems with orbitally non-degenerate ground states (mono-determinantal wavefunctions). In contrast, the applicability of the theory is severely limited in cases where a superposition of charge distributions described by several rather than one Slater determinants (multi-determinantal wavefunctions) is mandatory for a realistic description. Systems with orbital degeneracy, which are the subject of the present study, clearly fall into this latter category. In this context, we mention, but will not further discuss, pragmatic approaches that allow one to deduce ligand eld parameters from DFT calculations.31–34 Magnetic systems of the type considered here are still too large to be treated with the available implementations of variational conguration interaction (CI) type approaches that cover both static and dynamic correlation eﬀects. Even the application of complete active space self-consistent eld method (CASSCF)35 in conjunction with second-order perturbation corrections to the CASSCF energies (such as the complete active space perturbation theory, CASPT2,36–40 or the N-electron-Valence-Perturbation Theory NEVPT2 (ref. 40–44)) are very challenging to apply to

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article systems with more than one hundred atoms in conjunction with at least triple-zeta basis sets. The potential of using such approaches to calculate spin Hamiltonian parameters of mono-15,45–47 and bi-48–50 and even trinuclear transition metal complexes51 was recently demonstrated. Additionally, a general rst-principles method to calculate the spin-dependent part of the energies of ground and excited multiplets for larger polynuclear complexes was proposed.52 In this study, we apply the recent implementation of the CASSCF and NEVPT2 methods in the ORCA53,54 program package to perform large-scale correlated calculations on the electronic structure and magnetic properties of a series of complexes of high-spin FeII with linear FeX2 (1–5, 7) and bent FeN2 (6) cores (see ref. 29 and 55 for depictions of the structures of these molecules). This work was performed in parallel with an ongoing experimental study of their magnetic properties reported in the preceding companion paper.55 We use the protocol developed and applied for the interpretation, analysis, and prediction of the magnetic properties of the closely related series of [Fe(tpaR)] compounds published recently.46 The energies of the lowest spin-levels, which govern the magnetic behavior of the complexes, and their ligand eld analysis provide important insights into the respective inuences of chemical bonding and static and dynamic vibronic coupling on the observed spin-reversal barriers. This paper is divided into two parts. In the rst part, the basic theory and the computational scheme are outlined. These include the ligand eld background for analyzing the ab initio results and the static and dynamic vibronic coupling model employed for the interpretation of the magnetic data. In the second part, the results involving analysis of the chemical bonding, magnetic properties, and the ligand eld are described.

2

Computations and theory

2.1

Computations

The electronic energy levels for the complexes were computed using geometries from the crystal structures of 1 and 3,55 2,56 4 and 6,30 5,57 and 7.29 The computational protocol for the calculation of CASSCF/NEVPT2 wavefunctions/energies was previously described in ref. 55. The calculation of the magnetic properties—isothermal magnetizations and magnetic susceptibilities—using these wavefunctions and energies were

Fig. 1 Fe(CH3)2, Fe(NH2)2, and Fe(OH)2 DFT-optimized model complexes with D3d, D2h, and C2h geometries employed in the analysis of the FeII–ligand chemical bond and the pseudo Jahn–Teller activity of the d6 conﬁguration of FeII; Orange, gray, blue, red and cyan spheres represent Fe, C, N, O and H atoms, respectively.

This journal is ª The Royal Society of Chemistry 2013

Chemical Science detailed in a recent publication.46 In order to study vibronic coupling eﬀects, starting with complex 2, possessing trigonal symmetry and the pseudo Jahn–Teller eﬀect in complexes 1 and 3–7, we employed the truncated model complexes Fe(CH3)2, Fe(NH2)2 and Fe(OH)2 (see Fig. 1).

2.2

Ligand eld considerations 5

The E ground state of FeC2 (complex 2, accounting for the trigonal symmetry due to the next-nearest neighbors) is described by a total spin S ¼ 2 arising from two singly occupied orbitals e(dx2y2) or e(dxy) in addition to the half-lled d5 shell. These states give rise to ML ¼ 2 eigenfunctions of the angular ^z (eqn (1)). momentum operator L pﬃﬃﬃ 5 E; 2 ¼ 1= 2 5 E; dx2 y2 i5 E; dxy (1) Note that the states r5E,2i and r5E,2i cannot mix under the ^x and L ^y since ML changes by 1 unit of angular action of L ^x and L ^y. Mixing of these states with the momentum through L higher-lying 5E(dxz,yz)1 (ML ¼ 1), levels is possible. However, the latter are much higher in energy and will be neglected here. The eﬀects of these states on the magnetic properties will be discussed in Section 3.2.3 and 3.3. In this approximation, the spin–orbit ^ SOC assumes the form of eqn (2). coupling (SOC) operator H H^ SOC ¼ (z/4)L^zSˆz

(2)

^ SOC is represented by a diagonal 10 Within the rMS,MLi basis, H 10 matrix with elements (z/4)MSML (MS ¼ 0, 1, 2 and ML ¼ 2).58–61 The parameter z is the eﬀective one-electron SOC ‘constant’ for FeII (see ref. 17 and 62 for a detailed discussion). The energetic eﬀect of low-symmetry perturbations on the 5 E(dx2y2) and 5E(dxy) sublevels can be described in terms of two parameters d1 and d2 accounting for the splitting and mixing of 5 5 E dx2 y2 E dxy " # (3) d1 d2 H^ LF ¼ d2 d1 j2i " 5

5

j2i

0

d1 id2

d1 þ d2

0

#

(4)

these states as given by eqn (3). Following eqn (1), these sublevels can be transformed into a ML ¼ 2 basis (eqn (4)). The physical origin of d1 and d2 will be subject to a thorough ^ SOC + analysis in Sections 3.2.3 and 3.3. The Hamiltonian H ^ Z (H ^ Z ¼ the Zeeman operator) represented in the rML ¼ ^ LF + H H 2, MS ¼ 2, 1,0i basis, as well as energy and g-tensor expressions (normalized to a m ¼ 1/2 pseudo spin)25 are given in the ESI.† The [Fe(tpaR)] single-molecule magnets from ref. 22 and 23 possess trigonally elongated geometries and a 5 E(dxz,yz)1 ground state. Here, SOC leads to two lowest magnetic levels A1 and A2 which are split by the trigonal symmetry. Being an equal mixture of total angular momenta with MJ ¼ +3 and MJ ¼ 3, these states carry no magnetic moments. The Chem. Sci., 2013, 4, 139–156 | 141

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

complexes of the present study are completely diﬀerent. The ground state for linear complexes FeX2 is 5E(dxy,dx2y2)1 (complex 2, FeC2, can be ascribed as a trigonally compressed one), which under the action of SOC leads to a E(MJ ¼ 4) magnetic ground state. For both types of FeII-based singlemolecule magnets, and within the given approximation, pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ geometric distortions described by d ¼ d1 2 þ d2 2 s 0 do not cause a splitting of the MJ(MS s 0) pairs, leaving A1 and A2 in the former type of complexes accidentally degenerate. Quite diﬀerently, MJ levels with MS ¼ 0 undergo a rst-order splitting (2d) depending p onﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ the magnitude of the distortion (in ﬃ energetic sense, d ¼ d1 2 þ d2 2 s 0) but not on its direction (i.e., on 4, tg4 ¼ d2/d1). From eqn (1)–(4), the origin of the magnetic anisotropy arises; without oﬀ-axial distortions ﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðd ¼ d1 2 þ d2 2 ¼ 0Þ there is a 1 : 1 mixing between the |dx2y2i1 and |dxyi1 sublevels of the 5E term by SOC, and this leads to the addition of an orbital angular momentum of 2 mB to the net spin S ¼ 2 moment (4 mB). Focusing on the |MJ ¼ 4i ground state magnetic pair, an Ising-type anisotropy with gz ¼ 12 and gx,y ¼ 0 (d z) is obtained. In the limiting case of very large distortions (d [ z), the latter reduces to the spin-only values of gz ¼ gx ¼ gy ¼ 8. 2.3

The 5E53 Renner–Teller eﬀect

Unlike bent complex 6 and linear complex 7, the pseudolinear FeX2 cores in 1–5 possess inversion symmetry. Therefore, no linear vibronic coupling with the oﬀ-centric normal modes, 3, which serve to distort the linear geometry to a bent structure is possible. The energy lowering and energy splitting of the 5 E(dx2y2dxy)1 ground state of the FeII complexes due to Renner– Teller (RT) vibronic coupling is described by eqn (5),63–69 in which the nuclear coordinates Qx and Qy are components of the 3 mode (eqn (6)), r is the RT radius (eqn (7)), and 4 (eqn (8)) denes the direction of the distortion. 2 g 2 1 E ¼ K3 Qx 2 þ Qy 2 þ j Qx 2 þ Qy 2 Qx 2 þ Qy 2 2 2 1 2 4 ¼ ðK3 gÞr þ jr 2

Qx ¼ rcos 4; Qy ¼ rsin 4 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r ¼ Qx 2 þ Qy 2

(7)

tg4 ¼ Qy/Qx ¼ d2/d1

(8)

The parameters K3 and j describe the eﬀect of the harmonicity and anharmonicity, respectively (i.e., two terms due to forces which tend to preserve the linear geometry). The g-term quanties the vibronic force that leads to distortions and, accordingly to a splitting (g(Qx2 + Qy2)) of the 5E(dx2y2,dxy)1 ground state (eqn (5)). Depending on whether K3 > g or K3 < g, two diﬀerent situations are encountered (see Fig. 2). In the rst case, no new minima in the adiabatic ground state potential energy surface (APES) arise; however, the adiabatic approximation is violated by the vibronic mixing (via a term gQxQy) between the two sublevels. The other extreme, K3 < g, leads to a negative curvature for the lower surface, and therefore to dynamical instability. As a consequence, new minima on the APES corresponding to bent structures arise. Energy expressions, derived in the ESI,† allow us to relate the parameters K3, j, and g with the geometry of the minimum of the adiabatic ground state potential surface (APES) (rmin), the Renner–Teller stabilization energy ERT, and the energy of the vertical Franck–Condon transition EFC from the lower to the upper sheet of the APES (at the position of the minima) in terms of g, K3 and j. In turn, using these expressions g–K3 and j have been deduced from DFT values of rmin and ERT, obtained from a truncated FeC2 model complex (see Fig. 1). An estimate for K3 ¼ h- u3 is obtained using he corresponding Zn(CH3)2 analog, which lacks RT-activity. This leads to the parameters h- u3 ¼ 131 cm1, g ¼ 461 cm1, and j ¼ 8.2 cm1. Energy eigenvalues and eigenfunctions of vibronic levels were calculated using a Hamiltonian of the form: ^ vib + H ^ SOC + H ^ RT + H ^Z H^ ¼ H

(5)

(6)

(9)

^ vib including the with the harmonic vibrational Hamiltonian H ^ ^ RT, and H ^ Z, potential and kinetic energy terms and H SOC, H

Fig. 2 Variable adiabatic potential energy surface of a FeIIX2 complex with a doubly degenerate 5D ground state with respect to the oﬀ-centric displacement Qx in the case of the 5D5p Renner–Teller eﬀect: weak coupling – term splitting without instability (left); strong coupling – dynamic instability; nuclear probability distributions h|j|2i are shown with dotted lines.

142 | Chem. Sci., 2013, 4, 139–156

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

Chemical Science

representing the spin–orbit coupling, Renner–Teller, and Zeeman energy operators, respectively. The Hamiltonian of eqn (9) has been set up in the basis rJi of the products of electronic wavefunctions rfii ¼ rML ¼ 2, MS ¼ 2, 1, 0i, i ¼ 1 : 10 and 0 0 harmonic vibrational |cj(Qxi$|ck(Qyi wavefunctions up to level nvib (see ESI† for details). Isothermal magnetic susceptibilities and magnetizations were calculated employing the representa^ Z in the basis rJi and making explicit use of the tion of H calculated eigenvectors following procedures outlined previously.46

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

2.4

Ligand eld analysis of the ab initio results

Ab initio results were analyzed by mapping the ab initio multireference wavefunctions and energies onto ligand eld theory in the manner developed in detail in ref. 70. In this treatment, the LF Hamiltonian is viewed as an eﬀective Hamiltonian that acts on the subspace of states originating from a given dnconguration of a transition metal subject to perturbations from surrounding ligands. For an FeII center without including SOC, the d6 conguration spans 5, 45 and 50 electronic states with total spins of S ¼ 2, 1, and 0, respectively. The LF Hamiltonian within this basis is expressed in terms of a LF 5 5 matrix for one d-electron and atomic like parameters of interelectronic repulsion B and C. The energies of the ve S ¼ 2 states for FeII do not depend on the parameters B and C, and the LF matrix for the ve S ¼ 2 levels can be identied with the 5 5 LF matrix for one d-electron. From the possible parameterization oﬀered by the LFT, the angular overlap model (AOM) nds most favor among chemists.71–73 This model expresses the matrix elements of the 5 5 LF matrix in terms of parameters dened for well-aligned d-orbitals of s- and p-type, el (l ¼ s, pc, ps) multiplied by factors Flu(ql, 4l, jl) that depend solely on the angular geometry of the ligands (l, described by the Euler angles ql, 4l, jl). AOM energy expressions for a FeX2 complex with C2v symmetry (with a choice of Cartesian axes as shown in Fig. 3) have been derived and listed in the ESI.† The parameters es, epc, and eps quantify the energy destabilization of the FeII d-orbitals due to their negative overlap with the corresponding wellaligned ligand orbitals of s- and p-type (see Fig. 4), where

Fig. 4 Interactions approximating the FeII–ligand bond in FeN2 complexes 1, 3– 4, 6, and 7 (upper), FeO2 complex 5 (middle), and FeC2 complex 2 (lower), and their angular overlap model parameterizations.

anisotropy of the interactions of p-type, epc and eps, is taken into account (see Fig. 3 and 4 for the denition of the angle q and the AOM parameters, respectively). For a linear FeX2 complex (q ¼ 0 ) with dominating ligand donor functions of es > epc ¼ eps ¼ ep > 0, all parameters being positive in this case, the orbital energy order d(dx2y2, xy) < p(dxz,yz) < s(dz2) results:

e d dx2 y2 ;xy ¼ 0

(10) e p dxz;yz ¼ 2ep e½sðdz2 Þ ¼ 2es AOM parameters are traditionally deduced from a t to electronic d–d transitions observed in absorption and emission spectra of transition metal complexes. This procedure is oen (although not always) challenging, because the number of parameters is too large to allow for a unique determination. Recently, a procedure was proposed allowing one to deduce the LF parameters from ab initio calculations,70 which can be summarized as follows. First, focusing on the S ¼ 2 states, the 5 5 CI matrix in the basis of the Slater Determinants (SDs) built up from the metal-3d based molecular (CASSCF) orbitals is calculated. Focusing on SDs with MS ¼ S ¼ 2, we note that each single SD is a spin eigenfunction (i.e., SDs and conguration state functions (CSFs) are identical in this case). With the output of the electronic structure program, the CASSCF eigenvalues (EICASSCF) and eigenfunctions CCASSCF(1 : 5, I) (I ¼ 1 : 5) are directly available. Let us denote the diagonal matrix constructed from EICASSCF with LCASSCF(EICASSCF,I ¼ 1 : 5). We then deduce the LF matrix HLFT ¼ {HLFT IJ ,I,J ¼ 1 : 5} using the transformation: † HLFT CASSCF ¼ CCASSCFLCASSCFCCASSCF

Fig. 3 1–7.

Cartesian axes choice and geometrical parameters for the FeX2 core in

This journal is ª The Royal Society of Chemistry 2013

(11)

Dynamic correlation eﬀects are introduced via diagonal corrections to LCASSCF as provided by second-order many-body perturbation theory in form of the NEVPT2 method (DLNEVPT2, eqn (13)). The AOM parameters (pl) are then obtained by a leastsquares t based on eqn (14), where the matrices HAOM and HLFT NEVPT2 have been transformed into the traceless forms HAOM (pl) and HLFT b NEVPT2,b, respectively. Chem. Sci., 2013, 4, 139–156 | 143

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

† HLET NEVPT2 ¼ CCASSCFLNEVPT2CCASSCF

(12)

LNEVPT2 ¼ LCASSCF + DLNEVPT2

(13)

(pl) ¼ HLFT HAOM b NEVPT2,b

(14)

Adopting the one-electron parameters without changes, the parameters B and C were obtained from the computed energies of the spin–forbidden transitions, which, in the present case, are the transitions from the 5E ground state to the triplet ligand eld excited states. Finally, using es, ep, B, and C and switching on SOC, we x the value of z from the computed energies of the 5 E ground state SOC split sublevels. These calculations were performed through an interface between the ORCA program and the well-established ligand eld program package AOMX.74

3

Results and discussion

1, 3, 4, 6, and 7, with N-amido donors, there is a plane dened by N and the directly connected two atoms X forming N–X bonds; here X represents C and Si (1), C and H (3, 4, and 6), or two C atoms (7). As the FeII center is located in the same plane as the N(sp2)-donor atoms and their nearest neighbors, there is a well-dened direction for the p-interactions between FeII center (according to Fig. 4, the appropriate iron orbital is dyz) and the amido p-electron pair of the same symmetry (dened here as ps type in AOM). Since the Fe–N bond can be considered as weaker than the N–X bonds, we assign the local Fe–ligand bond a pseudosymmetry of C2v. Finally, in complex 5 there are two donor lone-pairs; one of these pairs, similar to Fe–N, has the symmetry appropriate for ps-type overlap with the out-ofthe Fe–O–C plane dyz orbital, while the other pair (located within the Fe–O–C plane) is available for pc-type overlap with the metal dxz orbital. This arrangement denes a local Cs pseudosymmetry.

3.1 Chemical bonding and vibronic activity of twocoordinate complexes of FeII It follows from X-ray data that the FeX2 cores in complexes 1–5 and 7 are linear. However, due to the nearest and next-nearest neighboring atoms of the FeII center, the electron density distribution deviates from idealized DNh symmetry. It has been shown that the second coordination sphere aﬀects metal– ligand bonding and results in dramatic changes to the color and magnetism of transition metals in solid matrices.75 Of immediate interest is the extent to which the next-nearest atoms in the coordination sphere of the FeII center aﬀect the magnetic properties of complexes 1–7. Depending on the number of strong bonds formed by the donor atoms C, N, or O (see Fig. 4), these complexes can be subdivided into three classes. With the C donor involved in three strong bonds to neighboring Si atoms, and neglecting hyperconjugation, there are no ligand orbitals available for FeII–C interactions of p-type in complex 2. The local symmetry around the Fe–C bond is C3v. In complexes

Table 1

Fig. 5 Molecular orbitals (DFT, PBE-functional) with contribution from the 3dorbitals of FeII as exempliﬁed using the Fe(NH2)2 model complex. From bottom to top, the s-interactions (left) are bonding and weakly and strongly antibonding, while the ps-interactions (right) are bonding and antibonding.

Molecular orbital energies and compositions characterizing the participation of the FeII orbitals in the bondinga

Fe(CH3)2

Fe(NH2)2

Fe(OH)2

s-type orbitals 7.45(bd): 11(4s) + 29(3dz2) [2] 5.40(weakly ab): 20(4s) + 50(3dz2) + 16(3dx2y2) [2] 5.37(nb): 4(4s) + 10(3dz2) + 10(3dxz) + 73(3dx2y2) [1] 0.32(ab): 47(4s) + 13(3dz2) [0]

s–pc type orbitals 9.55(bd): 8(4s) + 20(3dz2) [2] 4.91(weakly ab): 16(4s) + 48(3dz2) + 27(3dx2y2) [1] 4.06(nb): 8(4s) + 16(3dz2) + 72(3dx2y2) [1] 0.56(ab): 42(4s) + 15(3dz2) [0]

s–pc type orbitals 11.86(bd): 5(4s) + 12(3dz2) [2] 7.84(bd): 1(4s) + 6(3dz2) 5(4s) + 13(3dxz) [2]

p-type orbitals 5.69(nb): 86(3dxz) + 10(3dx2y2) [1] 5.65(nb): 95(3dyz) [1] d-type orbital 4.60(nb): 99(3dxy) [2]

ps-type orbitals 5.94(bd): 37(3dyz) [2] 3.58(ab): 66(3dyz) [1] pc-type orbital 4.88(nb): 96(3dxz) [1] d-type orbital 4.99(nb): 100(3dxy) [1]

5.24(weakly ab): 17(4s) + 57(3dz2) + 16(3dxz) + 3(3dx2y2) [1] 4.72(weakly ab): 7(4s) + 6(3dz2) + 71(3dxz) + 2(3dx2y2) [1] 4.33(nb): 2(4s) + 3(3dz2) + 95(3dx2y2) [2] 1.08(ab): 49(4s) + 17(3dz2) [0] ps-type orbitals 7.33(bd): 24(3dyz) [2] 4.38(ab): 78(3dyz) [1] d-type orbital 5.14(nb): 100(3dxy) [1]

a bd – bonding; ab – antibonding; nb – non-bonding; quasi restricted orbitals from DFT optimized model complexes (see ESI† for more details regarding these calculations); orbital electron occupation numbers are given in square brackets.

144 | Chem. Sci., 2013, 4, 139–156

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article

Chemical Science

Molecular orbital energies and Fe orbital percentages, deduced from quasi restricted DFT calculations performed on truncated Fe(CH3)2, Fe(NH2)2 and Fe(OH)2 model complexes (see Fig. 1) are listed in Table 1. Focusing on Fe(CH3)2, we note that, as expected, the Fe–C bonding is solely governed by strong Fe–C s-interactions, with the main participation coming from Fe 4s and 3dz2 orbitals; other orbitals (dxz, dyz, and dxy) are nonbonding due to a lack of ligand orbitals of appropriate symmetry. The interaction of the metal centered 3dz2 and 4s orbitals with the ligands gives rise to bonding, antibonding, and weakly antibonding MOs, as illustrated for Fe(NH2)2 at the le of Fig. 5. It is the intermixing of 4s into the nominally 3dz2 Fe-based orbital (as strong as 20% for Fe(CH3)2 and 16% for Fe(NH2)2) which converts this orbital from strongly antibonding (typical for octahedral complexes) to weakly antibonding in the FeX2 complexes 1–7. As will be shown below, this has an important eﬀect on the magnetic properties. In contrast to Fe(CH3)2, the out-of-plane type of p-bonding (ps) is essential in Fe(NH2)2 and Fe(OH)2. Here, a strong mixing between the FeII(dyz) and the corresponding ligand functions takes place, giving rise to the bonding and antibonding MOs, as illustrated for Fe(NH2)2 at the right in Fig. 5. The Cs symmetry of the Fe–O–H moiety leads to a mixing of the metal-based orbitals dz2, dxz, and dx2y2 (all behave totally symmetric with respect to the Fe–O–H symmetry plane). In a strictly linear complex, such as Cl–Fe–Cl, these orbitals would have s, pc, and dc character, respectively (see eqn (10)). However, based on the dz2, dxz, and dx2y2 FeII orbital percentages (57%, 71%, and 95% in the MOs with energies 5.24, 4.72 and 4.33 eV, respectively) the assignment given by the AOM (eqn (10)) is roughly correct. Linear (DNh) FeX2 complexes with a 5D(dx2y2,xy) ground state are intrinsically unstable with respect to geometric distortions since they are Renner–Teller active. Thus, bending of these complexes can cause the strictly non-bonding dx2y2,xy orbitals to become involved in bonding/antibonding interactions due to mixing of these orbitals with the p(dxz, yz) and s(dz2) orbitals and their ligands counterparts. The reduction in total energy is the driving force for such distortions. Calculating geometries from rst principles for such complexes is still far from trivial. First, at the point of orbital degeneracy and close to it, DFT is not applicable, while CASSCF is usually not accurate enough and many body perturbation approaches, such as NEVPT2, suﬀer from a lack of availability of analytic gradients, at least for larger molecules. Second, a ground state APES with two minima at distorted geometries is stationary at the point of degeneracy,

˚ bond angles in ), energy Table 2 Geometrical parameters (bond distances in A, stabilizations, Renner–Teller Radii rmin and C–M–C bending mode vibrational energies for Zn(CH3)2, Mn(CH3)2, and Fe(CH3)2 model complexes from DFT geometry optimizations

Zn(CH3)2 Mn(CH3)2 Fe(CH3)2

R

2(90 q)

E

rmin

n[d(X–Fe–X)] (cm1)

1.952 2.064 2.006

180 158.3 144.5

0 233 964

0 1.80 2.50

136 124 134

This journal is ª The Royal Society of Chemistry 2013

implying that the energy gradient at that point is zero. Therefore, while keeping to DFT, use of a distorted structure as the starting geometry in a geometry optimization is advisable. Third, the APES is highly anharmonic, implying the requirement of higher-order polynomials (up to order 8 for the cases studied below) in the Herzberg–Teller series66 expansion to model the energy of the 5D(dx2y2,xy) APES. DFT geometry optimizations of FeX2 (X ¼ CH3, NH2, and OH) starting from bent geometries resulted in a bent structure for Fe(CH3)2 with an X–Fe–X angle of 144.5 , but resulted in linear structures for Fe(NH2)2 and Fe(OH)2 (see Table 2). Based on a normal mode analysis, all geometrically optimized structures with linear FeX2 cores were calculated to be stable with respect to X–Fe–X bending. For the reasons stated previously (breakdown of the adiabatic approximation for closely-lying electronic levels), numerical values of the harmonic X–Fe–X frequencies are questionable. However, based on the very low values of these frequencies (see Table 2), they are still strongly indicative of so mode behavior. The quantication of the eﬀect of the latter on the magnetic properties will be analyzed below (see Section 3.2.2). A scan of the ground state energy versus the X–Fe–X angle for Fe(CH3)2 and the analogous Mn(CH3)2 and Zn(CH3)2 complexes with half lled (d5) and closed shell (d10) electronic congurations for the MII center, respectively, is shown in Fig. 6. To avoid the point of degeneracy, in these calculations X–M–X angles higher than 170 were excluded. A least-squares t to the data with a polynomial of degree 8 (solid lines in Fig. 6) allows one to deduce the energy of the linear geometry via interpolation. Remarkably, not only Fe(CH3)2 but also Mn(CH3)2 is stabilized by bending. It is interesting to note, that [FeCl2]+ (which is isoelectronic with Mn(CH3)2) is

Fig. 6 Adiabatic potential energy (in cm1) surfaces (APES) for M(CH3)2 (M ¼ Mn, Fe, Zn) model complexes, illustrating dynamical instabilities in the cases of Mn(CH3)2 (3d–4p pseudo Jahn–Teller coupling) and Fe(CH3)2 (3d–4p pseudo Jahn–Teller coupling superimposed by a (stronger) 5E53 Renner–Teller eﬀect). DFT optimized M–ligand bond distances are almost unchanged along the distortion path and have been ﬁxed at their values at the minimum of the APES (see Table 2). The APES has been constructed by varying the angle q (see Fig. 3 for its deﬁnition) between 45 and 80 in steps. Solid lines reproduce the data in terms of a polynomial of the degree 8: P(1)$Q8 + P(3)$Q6 + P(5)$Q4 + P(7)$Q2 + P(9) with the following values of the coeﬃcients P(1), P(3), P(5), P(7), and P(9): 0.0288, 1.7513, 43.0557, 362.0133, and 953 for Fe(CH3)2; 0.0181, 1.1037, 27.7868, 150.9680, and 232.8404 for Mn(CH3)2; 0.0514, 0.6800, 1.0285, 459.3716, and 234.2324 for Zn(CH3)2. Here, Q is expressed by the variable angle q at ﬁxed values of the metal–ligand bond distance R (from Table 2) according to Q ¼ 2R(90 q)(p/180).

Chem. Sci., 2013, 4, 139–156 | 145

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

calculated by DFT to be distorted as well, with an X–Fe–X angle of 132.2 and with an appreciably large stabilization energy of 1250 cm1. The origin of this eﬀect is found in the diﬀerent roles played by the 4px,y valence orbitals of FeII in the linear and bent congurations, respectively (see ESI†). Being non-bonding (due to their high energy separations from the ligand orbitals) and of diﬀerent parity (compared to 3d), the 4px,y AOs are essentially non-bonding in linear Mn(CH3)2. As illustrated in the ESI,† bending leads to a considerable mixing of 4px,y into 3dyz,xz, because both orbitals transform under the same irreducible representation in C2v. This mixing, or partial hybridization, leads to an increase of both s- and, to a lesser extent, ptype metal–ligand overlap. The eﬀect can be considered to be analogous to 3d–4s mixing for linear geometries but is energetically less pronounced. The extra electron in the dx2y2,xy orbital pair leads to an enhancement of the distortion (rmin) and an additional energy stabilization (E) as the comparison ˚ E ¼ 233 cm1) and between Mn(CH3)2 (rmin ¼ 1.80 A, ˚ E ¼ 964 cm1) shows (see Fig. 6 and Fe(CH3)2 (rmin ¼ 2.50 A, Table 2). Using data in Table 2, parameters of the vibronic coupling model were derived as specied in Section 2.3.

3.2

Electronic (vibronic) levels and magnetic properties

3.2.1 THE STATIC MODEL. The d6 conguration of the FeII centers in complexes 1–7 gives rise to 5 quintet states with NEVPT2 energies computed on the basis of the crystal structures listed in Table 3. The ground state of all complexes is a quintet 5E state with an energy that is lower by 15 200–20 600 cm1 than that of the lowest triplet state. The electronic absorption spectrum of 1 in 2-methyltetrahydrofuran consists of a broad asymmetric band centered at 8500 cm1 (see ESI†). Its simulation with two Gaussian envelopes led to the identication of the energies of the two expected d–d transitions centered at 7700 and 9400 cm1, respectively. These numbers compare well with the calculated CASSCF/

NEVPT2 transition energies (6936 and 10 062 cm1). We accordingly assign these as electronic transitions from 5 E(dx2y2,xy)1 to 5A1(dz2)1 and the 5E(dyz)1 split component of the 5 E(dyz,xz)1 state, with the lower energy transitions assigned to the 5E(dxz1) component and the even lower transitions within the 5E(dx2y2,xy)1 SOC sublevels manifold lying outside the spectrally accessible energy range. Deviations from axial symmetry (see Section 3.1) lead to a non-relativistic ground state splitting that is lowest for 2 (92 cm1) and increases from 4 (381 cm1) to 7 (766 cm1) and 6 (1246 cm1). The 5E ground state splitting for complexes 1, 3, and 5 (164, 241, and 222 cm1, respectively) are intermediate between those of 2 and 4 and thus lie outside the observed trend. This behavior will be analyzed below. The magnetic sublevels (classied according to the D3 symmetry encountered in complex 2) arising from the 5E ground state aer SOC are also included in Table 3. The ordering of these sublevels and their relative energy separations closely follows the energy expressions derived from a simplied treatment (see ESI†) in which only the in-state 5E SOC is considered. This behavior reects the dominant role of SOC, which widely suppresses low-symmetry splitting of all sublevels pairs with non-zero ML. In particular, splitting of the ground state magnetic sublevels |ML ¼ +2, MS ¼ +2i and |ML ¼ 2, MS ¼ 2i, through mixing with the topmost state |ML ¼ 2, MS ¼ +2i and |ML ¼ +2, MS ¼ 2i, respectively, is prevented by the large energy gap (2z z 800 cm1) between the two sublevels. This splitting is more pronounced for the rst excited states |ML ¼ +2, MS ¼ +1i and |ML ¼ 2, MS ¼ 1i, which interact with their respective |ML ¼ 2, MS ¼ +1i and |ML ¼ +2, MS ¼ 1i counterparts, because the former states are separated by a twofold smaller energy (z z 400 cm1). Being not aﬀected by SOC, the state E |ML ¼ 2, MS ¼ 0i is the only one that is strongly inuenced by oﬀ-axial distortions; its splitting is identical to that of non-relativistic 5E ground state (see Table 3). Using all of the SOC split sublevels of 5E ground state parentage and their associated wavefunctions, magnetizations

Table 3 Energies (in cm1) of S ¼ 2 states, of the lowest excited S ¼ 1 state (3A), and of the spin–orbit split components of the lowest 5E (D3 symmetry notations) from NEVPT2 calculations of linear FeX2 complexes with geometries from X-ray diﬀraction data and accounting for the complete set of the 5 quintet and 45 triplet electronic statesa

Electronic statea

1

2

3

4

5

6

7

5 E(dxy)1 (dx2y2)1 5 E(dxz)1 (dyz)1 5 A(dz2)1 3 A E(1)

0 164 3726 10 468 [9400] 7068 [7700] 18 023 0 0.002 189.8 190.4 322.8 485.8 612.8 625.0 810.1 810.3

0 92 4760 4799 5087 20 622 0 0.001 195.2 195.3 353.0 444.6 602.0 603.8 799.7 800.0

0 241 2080 8156 9190 14 944 0 0.013 176.4 179.8 286.6 529.1 632.0 646.6 822.0 822.5

0 381 2372 8057 9623 14 826 0 0.022 158.4 163.2 242.7 624.6 704.4 710.1 870.4 870.7

0 222 5004 7124 11 002 16 813 0 0.004 183.9 185.6 300.9 521.4 632.8 641.5 820.4 820.5

0 1246 8829 2409 9907 20 176 0 0.078 78.1 84.9 111.2 1347.5 1373.2 1384.4 1464.7 1464.8

0 766 6820 7649 8409 15 947 0 0.020 122.3 123.3 172.2 937.6 985.7 986.8 1106.7 1106.8

A1,A2(1) E(2) E(3) A1,A2(2) a

Experimental transition energies from near-IR d–d spectra of 1 are listed in square brackets.

146 | Chem. Sci., 2013, 4, 139–156

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article

Chemical Science

Fig. 7 Upper: experimental (blue squares) and calculated (NEVPT2, red circles) magnetic susceptibility data for complex 1 in the temperature range from 2 to 300 K under a static applied dc ﬁeld of 1000 Oe. Lower: experimental (squares) and calculated (NEVPT2, red circles) isothermal magnetization M vs. H/T for complex 1.

(M) and susceptibilities (cT) were calculated for 1–6. NEVPT2 values for cT and M for complexes 1 and 2 are both in good agreement with experimental data (see Fig. 7 and ESI†). The direct-current magnetization measurement at 1.85 K of the same crystalline sample as used for the M¨ ossbauer study28 yielded Mz ¼ 5.82 mB, which is very close to the NEVPT2 result (5.98 mB) for a sample of crystallites fully aligned with the applied magnetic eld. The experimental data given in ref. 55 are also in good agreement with the NEVPT2 result; however, here the NEVPT2 results have been converted to a powder average. The error for the data in ref. 28 is less than 3% away 0 from the maximal achievable magnetic moment of 6 mB (gMJ, 0 g ¼ 2, MJ ¼ 3). The situation changes for complexes 3–5 and 6. Here, the comparison between theory and experiment for cT and M (see

Table 4 and ESI†) shows that the calculated values are systematically larger than the experimental ones. The same complexes 3–5 display a drastic reduction (by as much as two to three orders of magnitude) in their relaxation times, as compared to 1 and 2.55 One could speculate that spin–orbit coupling (z), which is usually slightly overestimated in post Hartree–Fock calculations,46 might be responsible for the observed deviations. However, using empirically reduced values of z (accounting for the relativistic nephelauxetic eﬀect17 in the crudest possible way with an orbital reduction factor k) does not alleviate the problems. Thus, focusing on complex 3, both cT and M can only be brought into agreement with experiment by using an anomalously low orbital reduction factor k ¼ 0.6 (see ESI†). Hence, the deviations between theory and experiment must have a diﬀerent origin, as will be discussed in detail below. 3.2.2 DYNAMIC VIBRONIC COUPLING. From the preceding analysis it becomes clear that a model based on a static distortion is not able to account for the anomalously reduced magnetic moments reected in the measured susceptibilities and magnetizations of complexes 3–6. As detailed in Section 2.3, the 5E electronic state is vibronically unstable. In order to study the eﬀect of this instability on the magnetic properties, the energies and wavefunctions of the vibronic levels for the instate 5E53 vibronic coupling problem were computed utilizing the set of vibronic parameters K3 ¼ h- u, g and j adjusted to the ground state APES of Fe(CH3)2 (see Section 2.3). Variation of the vibronic coupling strength is accounted for in terms of the dimensionless parameter (f) which scales the Renner–Teller vibronic coupling constant g as well as the vibronic anharmonicity parameter j (f$g and f$j, respectively), while keeping the harmonic frequency of the 3 X–Fe–X bending mode (K3 ¼ h- u ¼ 131 cm1) unchanged. By increasing the value of f from 0 (static limit) to 1 (the strong coupling limit adjusted to the energy landscape pertaining to Fe(CH3)2), the eﬀect of the vibronic coupling strength on cT and M was systematically traced. Vibronic energy levels as functions of the parameters f are plotted in Fig. 8. Points at the le hand side of the diagram (f ¼ 0) correspond to energies of vibronic levels represented by basis functions built up as simple products of electronic |MJ ¼ ML + 0 0 MSi and vibrational |ck(Qx)cl(Qy)i parts, with energies of the uncoupled electron and nuclear motions given by eqn (15) (see ESI† for a visualization of the energy levels in this limiting case).

Table 4 Experimental and calculated (using molecular geometries from X-ray data, NEVPT2 results) values of the magnetic susceptibility (cT) and the isothermal magnetization (M) at 300 K and 2 K for complexes 1–6 (static model) and values of the vibronic coupling strength parameter f of a dynamic Renner–Teller model utilized to ﬁt the magnetic susceptibility data

Complex

1 Exp(calc.)

2 Exp(calc.)

3 Exp(calc.)

4 Exp(calc.)

5 Exp(calc.)

6 Exp(calc.)

(cT)300K f300K (cT)2K f2K MHTLFa MLTHFb

4.45(4.76) 0c 4.17(4.22) 0c 2.47(2.48) 3.00(3.00)

4.78(4.82) 0c 4.33(4.30) 0c 1.50(1.42) 3.24(3.04)

3.35(4.35) 0.133 3.73(4.80) 0.082 1.23(1.44) 2.74(3.10)

3.37(4.76) 0.132 2.88(4.30) 0.099 0.96(1.43) 2.14(3.11)

3.19(4.87) 0.162 2.87(4.46) 0.099 0.92(1.47) 2.06(3.15)

2.87(3.99) 2.03(3.44) 0.74(1.17) 1.93(2.88)

a MHTLF (high-temperature low-eld): T ¼ 5 K, H ¼ 1 T. b MLTHF (low-temperature high-eld): T ¼ 1.8 K, H ¼ 7 T. c Marks the appearance of a static limit corresponding to a value of f close to 0.

This journal is ª The Royal Society of Chemistry 2013

Chem. Sci., 2013, 4, 139–156 | 147

View Article Online

Chemical Science

Edge Article

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

decrease in the orbital contributions to the net magnetic moment and a concomitant change in the magnetic properties. From the energies and term assignments of the ve lowest magnetic levels (see Fig. 8, lower), we deduce that the level ordering (E < E < A1) in a dynamic Renner–Teller regime is completely diﬀerent than the one that applies in the static limit. In both cases the lowest sublevels remain doubly degenerate. Thus, the main diﬀerence is that the electronic degeneracy gives way to a vibronic one. One can qualitatively understand this behavior jML ¼ 2; MS ¼ 2; c0 ðQÞi jML ¼ H2; MS ¼ 2; c2 ðQÞi 3 2 1 1 pﬃﬃﬃ fg 7 6 2 hu3 z 7 2 2 6 7 6 7 6 7 4 1 5 pﬃﬃﬃ fg hu3 þ z 5 2 2 2 (16)

Fig. 8 Upper: vibronic energy levels from calculations on a Fe(CH3)2 model complex in the energy range below 900 cm1 versus the vibronic coupling strength parameter f scaling the vibronic parameters g ¼ 461 cm1 and j ¼ 8.19 cm1 of eqn (5). Lower: low energy range of the ﬁve lowest vibronic states responsible for the magnetic behavior (h- u3 ¼ 131 cm1). The ground state E(1) and the lowest excited state E(2) responsible for the energy barrier Ueﬀ of the Orbach relaxation mechanism are depicted in red.

through a two state model by restricting attention to a single interacting mode Q.63 Starting from the weak vibronic coupling limit (small f), the ground state is represented by |ML ¼ +2, MS ¼ +2, co(Q0 )i and |ML ¼ 2, MS ¼ 2, co(Q0 )i. These wavefunctions can only vibronically mix with |ML ¼ 2, MS ¼ +2, c2(Q0 )i and |ML ¼ +2, MS ¼ 2, c2(Q0 )i, respectively, as given by the matrix in eqn (16); here, co(Q0 )and c2(Q0 ) are the ground state and second excited state harmonic oscillator wavefunctions, respectively. For small f the separation between the two states (2(2 + h- u)) is large, while the mixing is small pﬃﬃﬃ (½ð1=2 2Þ fg 2ðz þ h- uÞ, Fig. 2, le). Thus, there are negligible contributions of the ML ¼ H2 orbital moments of opposite sign to the ground state magnetic pair ML ¼ 2. The probability distribution for the nuclear motion is close to Gaussian type |co(Q0 )|2 (see Fig. 2, le) with a maximum at the undistorted (linear) nuclear conguration. Let us now assume the other extreme: the strong Renner–Teller coupling limit of f ¼ 1. Here, there is nearly 1 : 1 mixing between the orbital moments ML ¼ +2 and ML ¼ 2, which are now better approximated by the |dx2y21i and |dxy1i spatial components and ground vibronic state described by two ground state 0 harmonic oscillator wavefunctions, displaced by 2Qo in congurational space relative to the undistorted geometry,

Fig. 9 Dependence of the z-components of the g-tensor in the lowest ﬁve thermally accessible magnetic states on the vibronic coupling strength parameter f.

E(MJ ¼ ML + MS,k, l) ¼ (z/4)MLMS + (k + l + 1)h- u

(15)

A mixing of these wavefunctions for non-zero f leads to the opening of a gap between the ve lowest levels and the other excited states (see Fig. 8, upper) and this gap increases with f. Thus, at values of f close to 0.1, a discontinuity in the spectrum of the magnetic excitations is predicted to occur. As illustrated by the dependence of the z-components of the g-tensor (see Fig. 9), the opening of the gap leads to a dramatic

148 | Chem. Sci., 2013, 4, 139–156

Fig. 10 Adiabatic potential energy surface in the strong coupling limit (f ¼ 1). The inversion splitting of spin–orbit vibronic levels rationalizing the reduction of the orbital magnetic moments is schematically presented.

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Edge Article

Chemical Science

Fig. 11 Calculated values of cT (H ¼ 1000 Oe) at 1.8 and 300 K as a function of the vibronic coupling parameter f.

E E dxy ; MS ¼ 2; c0 Q0 þ Q0 dx2 y2 ; MS ¼ 2; c0 Q0 Q0 o o 2 3 d1 izg0;0 þ d2 4 5 izg0;0 þ d2 d1 (17) 0

0

0

0

|dx2y2 ,MS ¼ 2,c0(Q Qo)i and ¼ 2,c0(Q + Qo)i (see Fig. 10). Being of the same energy (d1 ¼ 0), these two wavefunctions are now mixed to rst order by spin–orbit coupling through the matrix element izg0,0 (d2 ¼ 0), with g0,0 given by exp(Qo2) (eqn (17)). The latter describes the vibrational overlap 0 0 0 0 between two displaced c0(Q Qo) and c0(Q + Qo) ground state harmonic oscillator wavefunctions. Thus, the energy gap 2z, being of the order of 600–800 cm1 in a static limit, now becomes strongly reduced by the quantity g0,0 (the Ham reduction factor), which exponentially decreases with 0 increasing shis 2Qo. As illustrated by the dependence of cT on f (see Fig. 11, as well as the ESI† for a similar but less monotonic eﬀect on the magnetization), for intermediate Renner–Teller couplings, pﬃﬃﬃ which imply ð1=2 2Þfgz2ðz þ h- uÞ, Fig. 2, right), a discontinuous change of the vibronic wavefunction and reduction of the orbital momenta takes place. Under these conditions, the nominal ground rML ¼ 2,MS ¼ 2, c0(Q0 )i and excited rML ¼ 2,MS ¼ 2, c2(Q)i wavefunctions start to mix strongly, thus leading to large reductions of the orbital moments. Nuclear probability distributions also imply superposition between ground state harmonic wavefunctions (c0(Q0 )) with higher excited vibrational states (in the given illustration with the second harmonic c2(Q0 ), Fig. 2). This induces large amplitude motions and dynamic distortions. Such a behavior may not apply to the situation in the solid state where, due to crystal packing forces (d1, d2 in eq. 17 s 0), transitions from dynamically averaged distorted congurations to statically distorted structures can take place. This point of view is supported by the observation that the FeC2 core in complex 2 was reported to be linear, while a derivative with a bent FeC2 geometry in Fe(Ar)2 (C–Fe–C ¼ 159.34(6) ) has also been reported.57 Likewise, while a distorted X-ray structure of 6 was reported, the EPR spectrum of the same compound in solution is only compatible with a more linear complex.30 It is remarkable that by using this dynamic Renner–Teller coupling model, room temperature 1

|d1xy,MS

This journal is ª The Royal Society of Chemistry 2013

values of cT for complexes 2–5 could be tted with a single adjustable parameter f that is conned to the narrow range between f ¼ 0.142 0.015 (see Table 4). At lower temperatures, however, smaller values of f (0.082–0.099) were required to t the susceptibility. One would expect the inuence of vibronic coupling to scale with temperature, and therefore f should increase with increasing T. Likewise, at lower temperatures, one would expect the value of f to decrease in concert with the increasing inuence of the spin–orbit coupling, which attempts to mitigate the vibronic eﬀects in order to sustain the orbital angular momentum, a so-called inverse Jahn–Teller eﬀect.58–60 The proposed underlying nuclear dynamics of these linear X– Fe–X complexes would be expected to show up in the ellipsoids of thermal motion.76–79 An inspection of the low-temperature (T ¼ 90(2) K for 1 and 3–7 and 100(2) K for 2) structures of complexes 1–6 indeed lends support the notion of vibronic activity in the rst coordination sphere of the FeII centers. Temperature- and eld-dependent structural studies should give more detailed information about this interesting phenomenon. 3.2.3 NUCLEAR DYNAMICS, LOW SYMMETRY LIGAND FIELDS, AND MAGNETIC RELAXATION. A large reduction of the magnetic susceptibility and magnetization beyond the values predicted by the static model is also observed for complex 6 with a bent structure. Interestingly, it too shows anomalous thermal ellipsoids, similar to those encountered for 1–5.55 Following the concept of Section 3.2.2, we have to assume that some residual vibronic activity remains in the distorted FeN2 core of 6. Two critical remarks should be made regarding the quantitative aspects of the Renner–Teller model presented in Sections 2.3 and 3.2.2. First, as has been stated in Section 3.1, the actual symmetry of all complexes 1–7 is not DNh but lower, generally C1, and the electronic ground state, assumed to be electronically doubly degenerate (5E) is actually split. Thus, any vibronic activity of the kind discussed in Section 3.2.2 should be viewed as being of the pseudo Jahn–Teller type. Second, the actual molecular complexes are large and possess a huge number of degrees of freedom. Thus, many vibrations of 3-type may be involved in vibronic coupling, which leads to an unapproachable multimode dynamic pseudo Jahn–Teller coupling problem.

Fig. 12 Experimental cT data (H ¼ 1000 Oe) for complex 6 (red squares) and theoretical values calculated using a model80,81 accounting for the simultaneous presence of the low-symmetry ligand ﬁeld (strain) and vibronic coupling of variable strength f (where f ¼ 0 corresponds to the static limit of no vibronic coupling).

Chem. Sci., 2013, 4, 139–156 | 149

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

Employing complex 6 as a model and following the general theory of Ham,80,81 the eﬀect of the static distortion on the magnetic properties can be accounted for by considering vibronic coupling and lower symmetry ligand elds (strain) as independent perturbations. The latter is quantied by the strain energy matrix Hstrain deduced here directly from the mapping of the NEVPT2 results for the quintet state manifold onto ligand eld theory (see ESI†). The dependence of the magnetic susceptibility on the vibronic coupling strength under the strain inuence for complex 6 is depicted in Fig. 12. It follows from these results that the combined action of lowered symmetry and vibronic coupling have a crucial eﬀect in reducing the magnetic susceptibility from its static limit (with a calculated room temperature value of cT z 3.95 cm3K mol1 for f ¼ 0) to values closer (cT ¼ 3.05 cm3K mol1 for f ¼ 1) to the experimentally reported value of cT ¼ 2.87 cm3K mol1.55 The observed (and calculated) Curie–Weiss behavior of 6 results from the even population of the lowest lying vibronic energy levels (at 0.0, 0.051, 2.32, 3.05, and 3.61 cm1), which are well-separated from other excited vibronic spin states. The combination of reduced symmetry and vibronic coupling also has a crucial eﬀect on the magnetic relaxation time, s. Low-temperature (T ¼ 2 K) eld-dependent magnetic relaxation data have been used to quantify contributions to s from quantum tunneling (st) and direct relaxation (sd) mechanisms according to eqn (18) (ref. 55) (see Table 3 for a list of B1, B2, and AH2 deduced from a least square t to such data). Expressions connecting B1, B2, and A with tunnel-splitting of the ground state magnetic pair DE, the eﬀective g-tensor value along the easy direction (gz), and the 1 s1 ¼ s1 t þ sd ¼

B1 þ AH 2 T 1 þ B2 H 2

(18)

B1 ¼ DE2s1/2

(19)

B2 ¼ (bgzs1/2)2 2 3k Vs-ph gz b A¼ 2ph4 rvS 5

(20) (21)

Table 5 Intrinsic life-times (s1/2), tunnel-splitting energies (DE), and spin– phonon coupling parameters (Vs–ph) obtained from B1, B2, and A values deduced from the ﬁeld-dependent magnetic relaxation data for complexes 1–5 at 2 K

s1/2 (s) 1a 2b 3c 4d 5e

1.48 2.27 4.93 4.27 7.43

1010 1011 106 1011 107

DE (cm1)

Vs–ph (cm1)

so (s)1

Ueﬀ(cm1)1

6.93 107 5.10 107 0.002 2.85 106 0.003

0.017 0.024 0.045 0.078 0.133

1 1011 4 109 5 109 4 108 3 107

181 146 109 104 43

a gz ¼ 11.66, computed from CASSCF + NEVPT2 using the X-ray geometry and r ¼ 1.149 g cm3. b gz ¼ 11.95, computed from CASSCF + NEVPT2 using the X-ray geometry and r ¼ 1.118 g cm3. c gz ¼ 9.60, calculated with a dynamic vibronic coupling model using f ¼ 0.15 and r ¼ 1.182 g cm3. d gz ¼ 9.60, calculated with a dynamic vibronic coupling model using f ¼ 0.15 and r ¼ 1.127 g cm3. e gz ¼ 9.60, calculated with a dynamic vibronic coupling model using f ¼ 0.15 and r ¼ 1.203 g cm3.

150 | Chem. Sci., 2013, 4, 139–156

Fig. 13 Variation of the spin–phonon coupling parameter Vs–ph across the series from 1 to 5.

dipole–dipole spin–phonon coupling parameter, Vs–ph,82 respectively, are given in eqn (19)–(21). In addition, the intrinsic life time of the magnetic ground state level s1/2 (for B1 and B2), the sound velocity (vS), and the mass density r (for A) have been taken into account. Adopting a realistic value of 1.20 km s1 for vS,83 the mass density r from X-ray structures and the ab initio values of gz (static, 1–2, or vibronic, 3–5), s1/2, DE and Vs–ph were deduced (see Table 5) using the reported values B1, B2, and A (Table 3).55 There is no clear trend for the changes of s1/2 across the series 1– 6, which also diﬀer from the lifetimes so due to the thermally activated Orbach relaxation mechanism. Impressively, there is clear trend of the spin–phonon coupling parameter Vs–ph, which increases from 1 to 5 (see Fig. 13). With one exception, complex 4, the tunnel-splitting energy DE follows the same trend. It increases dramatically ongoing from 1 and 2 to complexes 3 and 5. Not unexpectedly, no relaxation time data could be recorded for complex 6. The low-symmetry ligand eld in this complex leads to a 1 : 1 mixing (via the matrix element of 475 cm1) between the |ML ¼ +2> and |ML ¼ 2> electronic levels, in addition to a mixing of |ML ¼ 0> in the |ML ¼ 2> pair due to mixing via the oﬀ-diagonal matrix element of 1602 cm1. Both eﬀects reduce the orbital moments and facilitate quantum tunneling of the magnetization. Similar eﬀects on the relaxation times for complexes 1–5 emerge from the plots of the corresponding matrix elements (see ESI†). A second eﬀect on the relaxation time at elevated temperature is due to the narrowing of the energy gap between the ground and the excited magnetic sublevels (see experimentally deduced values of Ueﬀ included in Table 5 in comparison with the energy gap between the energy levels marked with red circles in Fig. 8, lower). The anisotropy-reducing eﬀect of the low symmetry decreases on further symmetry lowering from nearly C2v (in 1, 3, and 4 with one lone pair) to C1 (in 5 with two lone pairs) and can be ascribed to bonding eﬀects arising from the next-nearest neighboring atoms of the FeII centers (see Section 3.3). We note, however, that the changes of these matrix elements across 1–6 are not monotonic and do not follow the observed trend in s across the series.55 The reasons for such diﬀerences may be twofold: (i) thermal ellipsoids of the L–Fe–L moieties (see Fig. S1† in ref. 55) show that contributions from vibronic coupling may be present in all complexes, and (ii) secondary interactions of the FeII center with next nearest neighboring C

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

Chemical Science

Table 6 Angular overlap parameters (in cm1) from an analysis of the multiplet energies calculated using NEVPT2 of FeX2 complexes 1–7 and the truncated linear model clusters FeL2 (L ¼ CH3, NH2, OH)

Parameter

1

2

3

4

5

6

7

Fe(CH3)2

Fe(NH2)2

Fe(OH)2

es eps epc s(AOM)a DE(5A1–5B1) E(5A1) s, pc E(5B1) ps

3351 5137 1828 349 442 660 248

2513 2364 2364 68 18 310 292

4418 3973 932 344 373 512 139

4512 3860 1018 464 346 497 151

5255 3397 2439 493 108 444 336

5291 3414 884 794 308 440 132

3977 4530 2321 189 291 607 316

1799 1757 1757 431 15 236 221

2478 5354 1454 223 519 717 198

3560 4478 2921 136 221 599 378

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

a

Standard deviations between calculated (using the listed set of AOM parameters) and NEVPT2 matrix elements within the quintet state manifold.

atoms might be important. This is particularly relevant in 3–6, where p-electron lobes due to C(sp2) atoms from the phenyl substituents make relatively short contacts providing s/p overlap to the FeII centers (Fe/C ¼ 2.588, 2.765, 2.792, and ˚ decreasing from 6 to 5 to 4 to 3, respectively). Such 2.817 A, interactions are absent in 1 and 2 where Fe–C(sp3) contacts ˚ in 1 and occur at much longer distances (2 3.621, 2 3.587 A ˚ 2 3.275, 2 3.369, and 2 3.504 A in 2). 3.3

Ligand eld analysis of the ab initio results

The AOM parameters es, epc, and eps derived from the CASSCF + NEVPT2 results are listed in Table 6. Compared to other studies,70 standard deviations between LF (calculated using the AOM parameter set) and ab initio matrix elements here are in the expected range and show the adequacy of the LF approach for the studied complexes. The AOM parameters are consistent with values resulting from the t of the spectrum of the linear complex FeCl2 (es ¼ 3500 cm1, ep ¼ 2300 cm1).84 The origin of the anomalously low calculated values of the parameter es (in particular for the FeC2 complex 2) originates from the stabilizing eﬀect of 4s–3d mixing, which reduces largely the Fe–X s-antibonding interactions in the nominally dz2 type MO (see Section 3.1). Because of this stabilizing eﬀect (and in contrast to the results obtained for the series of [Fe(tpaR)] complexes),22,23 a correlation between es and the Lewis ligand basicity is not observed (see ESI†). Thus, the lowest value of es in complex 2 (see Table 6) correlates with the greatest Lewis basicity for the C ligator. Table 6 also reports AOM parameters for the truncated model complexes Fe(CH3)2, Fe(NH2)2 and Fe(OH)2. From a comparison between the sets of parameters of the model complexes with those of 1–7, we can conclude that there is a signicant tuning of the ligand eld strength for each type of donor, C, N, and O, by the structure (substituents) of the extended ligand framework. As follows from the parameter ratio eps/epc [1, there is a large p-bonding anisotropy for the amido ligands in 1, 3, 4, 6, and 7, and the large values of eps characterize the amido ligands as strong p-donors. For N being involved in two strong bonds to neighbor atoms, there are no orbitals for p bonding in the Fe–NR2 plane. One should therefore expect epc to be zero. That this is not the case implies that there are large electrostatic contributions to the LF parameters for FeN2 complexes 1, 3, 4, 6, and 7. A similar conclusion can be

This journal is ª The Royal Society of Chemistry 2013

Fig. 14 Dependence of the quintet term energies on the distortion angle q (see Fig. 3) for linear complexes with FeC2 (C2v, top), FeN2 (C2v, middle), and FeO2 (C2h, lower) cores, as obtained using the set of parameters for complexes 2, 4, and 5, respectively (see Table 6).

made based on the non-zero eps ¼ epc ¼ ep parameters deduced from the ab initio results for complex 2 (compare with the zero overlap due to such kind of interaction emerging from Table 1).

Chem. Sci., 2013, 4, 139–156 | 151

View Article Online

Chemical Science

Edge Article

Table 7 Interelectronic repulsion (B and C) and spin–orbit coupling (z) parameters (in cm1) from an analysis of the multiplet energies calculated using NEVPT2 of FeX2 complexes (1–7)a

B C s(B, C) z s(z)

1

2

3

4

5

6

7

1512 3245 1012 413 44

1418 3564 402 407 2

970 3782 1003 426 66

822 3965 1072 459 114

1090 3734 952 420 60

602 4364 746 822 274

1833 3030 325 591 225

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

a

Standard deviations s between the energies of electronic multiplets, calculated using the given set of parameters B, C (deduced from a least squares t to energies of the ground state quintet to triplet excited states transitions) and z (from a least squares t to the spin– orbit split terms of the 5E ground state) and the NEVPT2 (B and C) and NEVPT2 + SOC (z) results.

It was pointed out in Section 3.1 that bonding anisotropy reduces the symmetry from approximately C3v (for 2 and Fe(CH3)2) to approximately C2v in the FeN2 cores of 1, 3, 4, 6, and 7. Values of the energy D(5A1–5B1) – the splitting between the upper and lower components of the 5E ground terms, were computed with AOM parameters (see Table 6) assuming an arbitrary but xed value of the angle q ¼ 15 . This energy correlates directly with the term g(Qx2 + Qy2) (see eqn (5)) and thus with the eﬀect of vibronic pseudo Jahn–Teller coupling on the magnetic anisotropy (Section 3.2). This can be seen in Fig. 14, which shows that the energies of 5A1 and 5B1 increase upon bending because the two states are being destabilized by s, pc, and ps antibonding interactions, respectively. Thus, the splitting D(5A1–5B1) appears as a combination of the eﬀects of s, pc, and ps antibonding interactions. Distortions also lead to a lowering of the orbital moments because of mixing of the 5A1(dz2 |2,0>) state into the 5A1 dx2y2 |2,2>+|2,2> state. In addition, s–d mixing further lowers 5A1(dz2) and contributes to the reduction of the orbital angular momentum. Finally, at acute values of the angle q, an avoided crossing leads to a switch from a 5A1(dx2y2) to a 5A1(dz2) electronic ground state. This switch quenches the orbital angular momentum (Table 7). The parameterization given by the AOM with diagonal energy terms described by s (for M(dz2)–X(pz)), in-plane (pc for M(dxz)– X(px)), and out-of-plane (ps for M(dyz)–X(py)) antibonding interactions between M and X, is only justied in complexes with strictly linear (epc ¼ eps ¼ ep) or two-fold (C2v) symmetry for each Fe–X fragment. This situation can change in complexes with composite ligands, where, say, carbon atoms attached to a given sp2-type N donor atom can aﬀect its lone pair from being optimally aligned for s-bonding with the metal. The physical implications of such bent bonds (or “misdirected valence”) have been discussed by Liehr in relation to the optical rotatory power in tri- and digonal dihedral compounds.85,86 As judged by the standard deviations in Table 6, the overall success of the standard LF model (where misdirected valence is neglected) with AOM parameters es, eps, and epc is quite high. Yet, as expected for complexes 5, 4, and the bent complex 6, all possessing Cs or even lower (C1) Fe–X pseudosymmetries, standard deviations (493, 464, and 794 cm1, respectively) are larger than for the

152 | Chem. Sci., 2013, 4, 139–156

complexes with the more regular structures: FeC2 (C3v, s ¼ 68 cm1) and, to a lesser extent, the FeN2 complexes 1, 3, and 7 (C2v, s ¼ 349, 344, and 189 cm1, respectively). The extra lone pair located in the Fe–O–R plane of the FeO2 complex 5 (see Fig. 4) has the proper symmetry for both s and pc overlap. Keeping to the linear O–Fe–O geometry, this is expected to create an oﬀ-diagonal matrix element hdz2rVlone_pairrdxzi ¼ 2espc and to aﬀect the nominal values of es and epc. As has been pointed out by Gerloch et al.,87,88 in the general case of a Fe–X bond with pseudosymmetry C1, up to six AOM parameters for a given ligand have to be introduced (extended AOM, diagonal es, eps, epc and oﬀ-diagonal espc, espc, epcs). While there is little hope in obtaining much insight from such an over-parameterized model (the data base from optical spectroscopy is too limited in order to unambiguously extract the model parameters; see ref. 87 and 88 for attempts to do this), it is worthwhile to reconsider the more complete ab initio results in the light of this concept. Numerical data (see ESI†) given by the 1 : 1 mapping of the ab initio NEVPT2 data onto LFT for complex 5 leads to the following conclusions: (i) There is full support from ab initio theory for the expected s–p mixing between the rddz2i and rddxzi orbitals. The energetic eﬀect of the C2v to the Cs symmetry lowering is calculated not to be very large (espc ¼ 420 cm1) but comparable to that of the symmetry lowering from Cs to C1 (rddxzi–rddyzi, epcs ¼ 409 cm1). (ii) Bonding anisotropy implicated by a lowered actual symmetry causes 5E(dx2y2, dxy) in-state mixing (edpc ¼ 217 cm1) and rst-order splitting (edc eds ¼ 138 cm1), eﬀects that are ignored in conventional AOM modeling. Such mixings are counterintuitive and must be electrostatic in origin. (iii) The largest oﬀ-diagonal terms are calculated between 5 E(dx2y2, dxy) and 5A1(dz2) (esdc ¼ 1302 cm1, esds ¼ 828 cm1), but are ignored in the extended AOM. These terms lead to a mixing of 5A1 into 5E(dx2y2, dxy) and thus reduce the orbital momenta (see above). However, the 5A1(dz2)–5E(dx2y2, dxy) energy separation is relatively large (10 483 cm1), which somewhat lessens this eﬀect. While not being favorable for the single-molecule magnet behavior of the considered complexes, spatial asymmetries leading to matrix elements of the type hdz2rVlone_pairrdxzi ¼ 2espc are responsible for chirality leading to natural circular dichroism (NCD) in chelate complexes with highly-symmetric MXn (n ¼ 2–6) cores. The combination of this property with that of a high-spin FeII center, providing coexistence of spatial asymmetry (chirality leading to a parity break) and magnetization (causing a break of time reversal symmetry) can lead to optically active magnets (or magneto-chirality) and to magnetochiral dichroism with non-polarized light.89 As magnetic chiral media are intrinsically magnetoelectric, electrical reading/ writing in the magnetic state is possible, a feature that is currently being pursued in the rising eld of molecular multiferroic materials. With a bistable ground magnetic state E and A1 and A2 excited states, as found in complexes 1–7, a combination with chirality in properly selected enantiopure derivatives seems a very promising direction for further exploration.

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

4

Conclusions

(1) CASSCF/NEVPT2 calculations of the electronic multiplets of two-coordinate FeII complexes with C, N, and O donor ligands have been used to analyze the bonding within complexes 1–7 and to trace the eﬀects of the next-nearest atoms to the metal center on the Fe-ligand bonds. Angular overlap model parameters deduced from ab initio data, along with DFT calculations performed on linear Fe(CH3)2, Fe(NH2)2, and Fe(OH)2 model complexes, demonstrate that the respective properties are strongly aﬀected by the supporting ligand scaﬀold (N(CSi) in 1, C(Si)3 in 2, N(HC) in 3, 4, and 6, O(C) in 5, and N(C)2 in 7). Due to these bonds, the approximate local Fe–X pseudosymmetry is lowered from C3v for Fe–C(sp2) to C2v for Fe–N(sp2) to Cs for Fe– O(sp), leaving one, two and three ligand lone pairs for bonding to FeII, respectively. The bonding anisotropy, increasing in this sequence, causes a splitting of the doubly degenerate ground and excited state levels assumed respectively as 5D(dx2y2, dxy) and 5P(dxz, dyz) for linear FeX2 complexes. (2) Spin orbit coupling, here accounted for by quasidegenerate perturbation theory (QDPT) in the basis of the non-relativistic CASSCF wavefunctions and diagonal NEVPT2 corrections to the CASSCF energies, leads to magnetic sublevels of 5E parentage. Low symmetry splitting of the doubly degenerate E ground state magnetic sublevel pair, caused by the bonding anisotropy, is strongly suppressed by SOC, but shows up to the full extent in the second doubly degenerate excited magnetic sublevel pair. Using static geometries taken from the crystal structures, low-temperature (T ¼ 1.8–5 K) isothermal magnetization data and magnetic susceptibilities (for 1 and 2) could be reasonably well reproduced. (3) A dynamic 5E53 vibronic coupling model of the Renner– Teller type has been employed to explain why the experimentally determined magnetization and susceptibility data for complexes 3–6 are systematically lower than the theoretically predicted results, assuming only static geometric distortions. The model incorporates three model parameters (g, j, and h- u3, corresponding to the Renner–Teller vibronic coupling constant, anharmonicity, and harmonic energy parameters, respectively) that were adjusted to the adiabatic ground state potential of a distorted Fe(CH3)2 model complex. Vibronic reductions of orbital contributions to the net magnetic moment exceed by far the orbital moment quenching induced by covalency. Following this model, it was possible to t the low (T ¼ 2 K) and room (T ¼ 300 K) temperature magnetic susceptibility data for complexes 2–6 in terms of a single parameter f, the vibronic coupling strength, which can vary between 0 (no vibronic coupling) and 1 (strong vibronic coupling). The best t values for f fall into a narrow range at 0.142 0.015. The given range of f nearly coincides with borderline of a discontinuous change from weak (f < 0.1) to strongly (f > 0.1) coupled electronic and nuclear motions, where vibronic coupling is being quenched by SOC (f < 0.1) or vice versa (f > 0.1). It is conceivable that in a solid, large amplitude movements will readily drive the system from a dynamically averaged into a static distorted nuclear conguration. The very diﬀerent magnetic behaviors reported for complexes 1–2 and 3–6 are a clear manifestation of such

This journal is ª The Royal Society of Chemistry 2013

Chemical Science behavior, and should be the subject of more detailed structural, magnetic, and spectroscopic studies. (4) A general method allowing a 1 : 1 mapping of the ligand eld matrix, as deduced from ab initio CASSCF + NEVPT2 calculations, onto corresponding AOM energy expressions was used to obtain values of the antibonding energies of s (es), the in- (epc) and out-of- (eps) plane p-type. The parameters show: (i) a large reduction of es due to 3dz2–4s mixing (hybridization) typical for linear X–M–X transition metal complexes, (ii) pbonding anisotropy reected in eps > epc for the Fe–N(sp2) and Fe–O(sp) type complexes, and (iii) framework hyperconjugative eﬀects manifested in values of ep assumed otherwise to be zero (ep for C(sp3) and epc for N(sp2)). In the same context, ligand eld matrix elements neglected in common AOM parameterization schemes, but accounted for by its extended versions (such as s–p mixings and misdirected valence) could be traced back and veried. Other couplings (dx2y2–dz2, dxy–dz2, and dxy– dx2y2), which, due to the high level of over-parameterization have not been discussed before, emerged from our analysis. (5) Based on the theoretical analysis, the following guidelines for generating new single-molecule magnets with improved magnetic anisotropies and relaxation times can be formulated: (i) enhancement of the spin–orbit coupling and concomitant suppression of the vibronic coupling is predicted to improve the anisotropy barrier Ueﬀ (see Fig. 8). Both features can be met by replacing the C, N, or O donor atoms with their heavier analogues, such as Si, P, or S. Indeed, some FeS2 moieties have already been reported.90 Ligand spin–orbit coupling, increasing in this direction may add to the metal one, thus compensating for the enhanced metal–ligand covalence, which tends to act in the opposite direction (relativistic nephelauxetic eﬀect). Such an increase in molecular magnetic anisotropy as a result of the coordination of increasingly heavier ligand atoms has been demonstrated recently in octahedral complexes of CrIII.91 Additionally, vibronic coupling, which decreases with increasing metal–ligand covalency, is expected to support a larger Ueﬀ. A nice manifestation of such an eﬀect is a recently reported CoS4 single-molecule magnet, the rst example of a transition metal complex exhibiting slow magnetic relaxation under zero applied dc magnetic eld.92 (ii) Metal–ligand bonds with C3v and C2v local pseudosymmetries, enforced by the next-nearest metal neighbors (C(sp3) and N(sp2)), are preferable to lower symmetry ones (O(sp2)), which create large matrix elements between the ground state MJ sublevels. (iii) Avoiding secondary metal–ligand interactions through the use of sterically encumbering ligands with aliphatic (1, 2) rather than aromatic substituents (3–5) has a favorable eﬀect on the relaxation time. Along the same line, bulky ligands of the former type tend to support linear FeX2 cores and thus oppose in an indirect way unfavorable vibronic coupling. (iv) Suppression of dipolar spin–spin interactions between magnetic centers in the solid will increase the relaxation time for the direct process. It is this kind of interaction which shows the expected trend of relaxation times (see Fig. 13) across the series. Thus decoupling of the molecule from the lattice is an

Chem. Sci., 2013, 4, 139–156 | 153

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science important goal. Aside from the usual approaches used to achieve this (e.g., dilution of the single-molecule magnets by substitution in a diamagnetic isomorphic compound or in frozen solution), stabilization of the molecules on a metal (usually gold) surface provides a modern way of approaching this. One possibility of doing this is given by using appropriately chosen spacer molecules that can “wire” a single-molecule magnet to a gold surface.1 Another method, involving vapor deposition, should be facile for certain mononuclear transition metal complexes that are neutral and can sublime. For example, complex 2 is easily sublimable.93 In the context of the FeX2 single-molecule magnets, a possible target would be an – AuS3C–C^C–Fe–C^C–CS3Au – structure. Unfavorable vibronic coupling which tends to stabilize bent structures will be suppressed within the constraints given above. (6) The large magnetic anisotropy due to unquenched rst order orbital momentum in the 5E ground states of the considered FeX2 complexes leads to large anisotropy barriers. However, quantum tunneling of the magnetization is particularly eﬃcient owing to the small value of S ¼ 2 and the lowsymmetry perturbations of the kind discussed in Sections 3.2.3 and 3.3. Thus, the search for better single-molecule magnets that stay magnetized at elevated temperatures requires a combination of a large Ueﬀ and a small quantum tunneling rate. This goal is only partly (due to intrinsic transversal magnetic elds stemming from dipole–dipole interactions which cannot be avoided in a solid) achieved by choosing Kramers rather than non-Kramers Fe(II) (S ¼ 2) ions, as was shown in the recently reported [Co(SPh)4]2 (S ¼ 3/2) complex.92 The condition of larger Ueﬀ (large/small spin–orbit/vibronic coupling) and a small quantum tunneling of the magnetization (large total moments MJ) seems to be ideally met in complexes of rare earths such as phthalocyanine (pc) double decker complexes, e.g. (pc)2TbIII.94 A similar possibility for complexes of 3d metals employs low-coordinate Fe(II) (introducing large Ueﬀ) ferromagnetically coupled with several MnII (S ¼ 5/2, introducing a large spin). Such a synthetic strategy has yet to be explored.

Acknowledgements This research was supported by NSF grant CHE-1111900. We thank Tyco Electronics for fellowship support of J.M.Z.

Notes and references 1 M. Mannini, F. Pineider, P. Sainctavit, C. Danieli, E. Otero, C. Sciancalepore, A. M. Talarico, M.-A. Arrio, A. Cornia, D. Gatteschi and R. Sessoli, Nat. Mater., 2009, 8, 194. 2 M. N. Leuenberger and D. Loss, Nature, 2001, 410, 789. 3 A. Ardavan, O. Rival, J. J. L. Morton, S. J. Blundell, A. M. Tyryshkin, G. A. Timco and R. E. P. Winpenny, Phys. Rev. Lett., 2007, 98, 057201. 4 P. C. E. Stamp and A. Gaita-Ari~ no, J. Mater. Chem., 2009, 19, 1718. 5 F. Torres, J. M. Hern´ andez, X. Bohigas and J. Tejada, Appl. Phys. Lett., 2000, 77, 3248.

154 | Chem. Sci., 2013, 4, 139–156

Edge Article 6 R. Sessoli, D. Gatteschi, A. Caneschi and M. A. Novak, Nature, 1993, 365, 141. 7 D. Gatteschi, R. Sessoli and J. Villain, Molecular Nanomagnets, Oxford University Press, New York, 2006 and references therein. 8 N. E. Chakov, S.-C. Lee, A. G. Harter, P. L. Kuhns, A. P. Reyes, S. O. Hill, N. S. Dalal, W. Wernsdorfer, K. Abboud and G. Christou, J. Am. Chem. Soc., 2006, 128, 6975. 9 C. J. Milios, A. Vinslava, W. Wernsdorfer, S. Moggach, S. Parsons, S. P. Perlepes, G. Christou and E. K. Brechin, J. Am. Chem. Soc., 2007, 129, 2754. 10 C. Sangregorio, T. Ohm, C. Paulsen, R. Sessoli and D. Gatteschi, Phys. Rev. Lett., 1997, 78, 4645. 11 S. M. J. Aubin, N. R. Dilley, L. Pardi, J. Krzystek, M. W. Wemple, L.-C. Brunel, M. B. Maple, G. Christou and D. N. Hendrickson, J. Am. Chem. Soc., 1998, 120, 4991. 12 A.-L. Barra, A. Canneschi, A. Cornia, F. Fabrizi de Biani, D. Gatteschi, C. Sangregorio, R. Sessoli and L. Sorace, J. Am. Chem. Soc., 1999, 121, 5302. 13 S. Accorsi, A. L. Barra, A. Caneschi, G. Chastanet, A. Cornia, A. C. Fabretti, D. Gatteschi, C. Mortal` o, E. Olvieri, F. Parenti, R. Sessoli, L. Sorace, W. Wernsdorfer and L. Zobbi, J. Am. Chem. Soc., 2006, 128, 4742. 14 L. Gregoli, C. Danieli, A.-L. Barra, P. Neugebauer, G. Pellegrino, G. Poneti, R. Sessoli and A. Cornia, Chem.– Eur. J., 2009, 15, 6456. 15 F. Neese and D. A. Pantazis, Faraday Discuss., 2011, 148, 229. 16 O. Waldmann, Inorg. Chem., 2007, 46, 10035. 17 F. Neese and E. I. Solomon, Inorg. Chem., 1998, 37, 6568. 18 C. J. Milios, C. P. Raptopoulou, A. Terzis, F. Lloret, R. Vincente, S. P. Perlepes and A. Escuer, Angew. Chem., Int. Ed., 2004, 43, 210. 19 E. K. Brechin, C. Boskovic, W. Wernsdorfer, J. Yoo, A. Yamaguchi, E. C. Sa~ nudo, T. R. Concolino, A. L. Rheingold, H. Ishimoto, D. N. Hendrickson and G. Christou, J. Am. Chem. Soc., 2002, 124, 9710. 20 J. Villain, F. Hartman-Boutron, R. Sessoli and A. Rettori, Europhys. Lett., 1994, 27, 159. 21 W. H. Harman and C. J. Chang, J. Am. Chem. Soc., 2007, 129, 15128. 22 D. E. Freedman, W. H. Harman, T. D. Harris, G. J. Long, C. J. Chang and J. R. Long, J. Am. Chem. Soc., 2010, 132, 1224. 23 W. H. Harman, T. D. Harris, D. E. Freedman, H. Fong, A. Chang, J. D. Rinehart, A. Ozarowski, M. T. Sougrati, F. Grandjean, G. J. Long, J. R. Long and C. J. Chang, J. Am. Chem. Soc., 2010, 132, 18115. 24 Throughout this work electron congurations due to the high-spin Fe(II) d6 subshell will be denoted by orbitals which carry the extra electron in addition to the half-lled d5 shell. 0 25 A diﬀerent denition of MJ ¼ MS + ML/2, used to directly relate the magnetic moment with the free electron go ¼ 2 0 value (M ¼ mBgoMJH), was employed in ref. 46. Here, we return to the usual denition of MJ ¼ MS + ML which also correctly reects the transformation symmetry of the

This journal is ª The Royal Society of Chemistry 2013

View Article Online

Edge Article

26 27 28

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

29

30

31 32 33 34

35 36 37 38 39

40 41 42 43 44 45 46 47 48

wavefunction. Another denition treating the total moment in a S ¼ 1/2 pseudospin approach (used by the ESR community) denes the magnetic moment as M ¼ 0 mBmgeﬀH (geﬀ ¼ goSMJ, m ¼ 1/2). B. R. McGarvey and J. Telser, Inorg. Chem., 2012, 51, 6000. D. Dai and M.-H. Whangbo, Inorg. Chem., 2005, 44, 4407. W. M. Reiﬀ, A. M. LaPointe and E. H. Witten, J. Am. Chem. Soc., 2004, 126, 10206. W. M. Reiﬀ, C. E. Schulz, M.-H. Whangbo, J. I. Seo, Y. S. Lee, G. R. Potratz, C. W. Spicer and G. S. Girolami, J. Am. Chem. Soc., 2009, 131, 404. W. A. Merrill, T. A. Stich, M. Brynda, G. J. Yeagle, J. C. Fettinger, R. De Hont, W. M. Reiﬀ, C. E. Schulz, R. D. Britt and P. P. Power, J. Am. Chem. Soc., 2009, 131, 12693. M. Atanasov, P. Comba and C. A. Daul, Inorg. Chem., 2008, 47, 2449. M. Atanasov, C. A. Daul and C. Rauzy, Struct. Bonding, 2004, 106, 97. M. Atanasov, C. A. Daul and C. Rauzy, Chem. Phys. Lett., 2003, 367, 737. M. Atanasov and P. Comba, in The Jahn-Teller Eﬀect: Fundamentals and Implications for Physics and Chemistry, ed. H. K¨ oppel, H. Barentzen and D. R. Yarkony, Springer Series in Chemical Physics, Berlin, 2009, p. 97. ˚ Malmqvist and B. O. Roos, Chem. Phys. Lett., 1989, 155, P.-A. 189. K. Wolinski and P. Pulay, J. Chem. Phys., 1989, 90, 3647. ˚ Malmqvist, B. O. Roos, A. J. Sadlej and K. Andersson, P.-A. K. Wolinski, J. Phys. Chem., 1990, 94, 5483. ˚ Malmqvist and B. O. Roos, J. Chem. Phys., K. Andersson, P.-A. 1992, 96, 1218. ˚ Malmqvist, P. L. SerranoB. O. Roos, M. P. F¨ ulscher, P.-A. Andr´ es, and M. Merch´ an, Theoretical Studies of the Electronic Spectra of Organic Molecules, in Quantum Mechanical Electronic Structure Calculations with Chemical Accuracy, ed. S. R. Langhoﬀ, Kluwer, Dordrecht, 1994. ˚ Malmqvist, Phys. Chem. Chem. Phys., B. O. Roos and P.-A. 2004, 6, 2919. C. Angeli, R. Cimiraglia and J.-P. Malrieu, Chem. Phys. Lett., 2001, 350, 297. C. Angeli, R. Cimiraglia, S. Evangelisti, T. Leininger and J.-P. Malrieu, J. Chem. Phys., 2001, 114, 10252. C. Angeli, R. Cimiraglia and J.-P. Malrieu, J. Chem. Phys., 2002, 117, 9138. C. Angeli, B. Bories, A. Cavallini and R. Cimiraglia, J. Chem. Phys., 2006, 124, 054108. R. Maurice, C. de Graaf and N. Guih´ ery, J. Chem. Phys., 2010, 133, 084307. M. Atanasov, D. Ganyushin, D. A. Pantazis, K. Sivalingam and F. Neese, Inorg. Chem., 2011, 50, 7640. D. Maganas, S. Sottini, P. Kyritsis, E. J. J. Groenen and F. Neese, Inorg. Chem., 2011, 50, 8741. R. Maurice, R. Bastardis, C. de Graaf, N. Suaud, T. Mallah and N. Guih´ ery, J. Chem. Theory Comput., 2009, 5, 2977.

This journal is ª The Royal Society of Chemistry 2013

Chemical Science 49 R. Maurice, N. Guih´ ery and C. de Graaf, J. Chem. Theory Comput., 2010, 6, 55. 50 R. Maurice, A. M. Pradipto, N. Guih´ ery, R. Broer and C. de Graaf, J. Chem. Theory Comput., 2010, 6, 3092. 51 S. Vancoillie, J. Chalupsk´y, U. Ryde, E. I. Solomon, K. Pierloot, F. Neese and L. Rulȋˇsek, J. Phys. Chem. B, 2010, 114, 7692. 52 M. Atanasov and P. Comba, in Structure and Function, ed. P. Comba, Springer, 2010, pp. 74–79. 53 F. Neese, WIREs Comput. Mol. Sci., 2012, 2, 73. 54 ORCA, An ab initio, DFT and Semiempirical SCF-MO Package – Version 2.8, 20 September 2010by F. Neese, F. Wennmohs, with contributions from U. Becker, D. Bykov, D. Ganyushin, A. Hansen, R. Izsak, D. G. Liakos, C. Kollmar, S. Kossmann, D. A. Pantazis, T. Petrenko, C. Reimann, C. Riplinger, M. Roemelt, B. Sandh¨ ofer, I. Schapiro, K. Sivalingam, E. Valeev and B. Wezisla, Max-Planck Institut f¨ ur Chemische Energiekonversion, http://www.mpibac.mpg.de/bac/index_ en.php. 55 J. M. Zadrozny, M. Atanasov, A. M. Bryan, C.-Y. Lin, B. D. Rekken, P. P. Power, F. Neese and J. R. Long, Chem. Sci., 2012, DOI: 10.1039/c2sc20801f. 56 T. Vieaus, W. Schwarz, K. H¨ ubler, K. Locke and J. Weidlein, Z. Anorg. Allg. Chem., 2001, 627, 715. 57 C. Ni and P. P. Power, Chem. Commun., 2009, 5543. 58 R. S. Fishman and F. A. Reboredo, Phys. Rev. Lett., 2007, 99, 217203-1. 59 R. S. Fishman, S. Okamoto and F. A. Reboredo, Phys. Rev. Lett., 2008, 101, 116402-1. 60 R. S. Fishman and F. A. Reboredo, Phys. Rev. B: Condens. Matter Mater. Phys., 2008, 77, 144421. 61 P. Reis, R. S. Fishman, F. A. Reboredo and J. Moreno, Phys. Rev. B, 2008, 77, 174433. 62 F. Neese and E. I. Solomon, in Magnetism: Molecules to Materials, ed. J. S. Miller and M. Drillon, Wiley-VCH, Weinheim, 2003, vol. IV, pp. 345–466. 63 I. B. Bersuker, The Jahn–Teller Eﬀect and Vibronic Interactions in Modern Chemistry, Plenum Press, New York and London, 1984. 64 I. B. Bersuker, The Jahn–Teller Eﬀect, University Press, Cambridge, 2006. 65 E. Renner, Z. Phys., 1934, 92, 172. 66 G. Herzberg and E. Teller, Z. Phys. Chem., Abt. B, 1933, 21, 410. 67 J. A. Pople and H. C. Longuet-Higgins, Mol. Phys., 1958, 1, 372. 68 R. N. Dixon, Mol. Phys., 1965, 9, 357. 69 A. A. Petelin, Int. J. Quantum Chem., 1972, 6, 701. 70 M. Atanasov, D. Ganyushin, K. Sivalingam and F. Neese, Struct. Bonding, 2012, 143, 149. 71 C. K. Jørgensen, R. Pappalardo and H.-H. Schmidtke, J. Chem. Phys., 1963, 39, 1422. 72 C. E. Sch¨ aﬀer and C. K. Jørgensen, Mol. Phys., 1965, 9, 401. 73 B. N. Figgis and M. A. Hitchman, Ligand Field Theory and Its Applications, Wiley-VCH, NewYork, 2000. 74 H. Adamsky, with contributions from P. E. Hoggard, M. Atanasov and K. Eifert, AOMX, http://www.aomx.de.

Chem. Sci., 2013, 4, 139–156 | 155

View Article Online

Downloaded on 18 March 2013 Published on 25 October 2012 on http://pubs.rsc.org | doi:10.1039/C2SC21394J

Chemical Science

Edge Article

75 D. Reinen, M. Atanasov and S.-L. Lee, Coord. Chem. Rev., 1998, 175, 91. 76 J. D. Dunitz and D. N. J. White, Acta Crystallogr., Sect. A: Cryst. Phys., Diﬀr., Theor. Gen. Crystallogr., 1973, A29, 93. 77 J. D. Dunitz, E. F. Maverick and K. N. Trueblood, Angew. Chem., 1988, 100, 910. 78 J. H. Ammeter, H. B. B¨ urgi, E. Gamp, V. Meyer-Sandrin and W. P. Jensen, Inorg. Chem., 1979, 18, 733. 79 M. Atanasov, W. K¨ onig, H. Craubner and D. Reinen, New. J. Chem., 1993, 17, 115. 80 F. S. Ham, in Electron Paramagnetic Resonance, ed. S. Geschwind, Plenum Press, New York, 1972, p. 1. 81 F. S. Ham, Phys. Rev., 1965, 138, 1727. 82 Vs–ph is related with the magnetogyric ratio for electrons, Nneigbors P 6 . 2 n – a ro;i g ¼ e/mc, the parameter a ¼ 2 i¼1

constant somewhat greater than unity, the magnetic pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ moment per ion m ¼ gJ Jð J þ 1Þ (in Bohr magnetons) and n –the number of magnetic ions per 1 volume as Vs–ph2 ¼ (3a/8)g2n2m2h- 2, A. Abragam and B. Bleaney, Electron Paramagnetic Resonance of Transition Ions, Clarendon Press, Oxford, 1970.

156 | Chem. Sci., 2013, 4, 139–156

83 V. Starovoitova, G. R. A. Wyllie, W. R. Scheidt, W. Sturhan, E. Ercan Alp and S. M. Durbin, J. Phys. Chem. B, 2008, 112, 12661. 84 C. W. DeKock and D. M. Gruen, J. Chem. Phys., 1966, 44, 4383. 85 A. D. Liehr, J. Phys. Chem., 1964, 68, 665. 86 A. D. Liehr, J. Phys. Chem., 1964, 68, 3629. 87 M. Gerloch, J. H. Harding and G. G. Woolley, Struct. Bonding, 1981, 46, 1. 88 A. J. Bridgeman and M. Gerloch, Prog. Inorg. Chem., 1997, 45, 179–281, p. 238, Table III. 89 C. Train, R. Gheorghe, V. Krstic, L.-M. Chamoreau, N. S. Ovanesyan, G. L. J. A. Rikken, M. Gruselle and M. Verdaguer, Nat. Mater., 2008, 7, 729. 90 T. Nguyen, A. Panda, M. M. Olmstead, A. F. Richards, M. Stender, M. Brynda and P. P. Power, J. Am. Chem. Soc., 2005, 127, 8545. 91 H. I. Karunadasa, K. D. Arquero, L. A. Berben and J. R. Long, Inorg. Chem., 2010, 49, 4738. 92 J. M. Zadrozny and J. R. Long, J. Am. Chem. Soc., 2011, 133, 20732. 93 A. M. LaPointe, Inorg. Chim. Acta, 2003, 345, 359. 94 N. Ishikawa, Struct. Bonding, 2010, 135, 211 and references therein.

This journal is ª The Royal Society of Chemistry 2013